 
data_358d
#CSD 428355
#complex Cs2K10-1 
_audit_creation_method           SHELXL-2013
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'H30.80 Cs2 K10 Nb12 O65.40 Pt2'
_chemical_formula_weight         3239.36

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -2.0727 0.6215 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pt Pt -1.7033 8.3905 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   10.5213(16)
_cell_length_b                   12.6202(19)
_cell_length_c                   15.122(2)
_cell_angle_alpha                96.136(4)
_cell_angle_beta                 98.791(4)
_cell_angle_gamma                96.912(5)
_cell_volume                     1953.7(5)
_cell_formula_units_Z            1
_cell_measurement_temperature    150(2)
_cell_measurement_reflns_used    5562
_cell_measurement_theta_min      2.21
_cell_measurement_theta_max      26.55

_exptl_crystal_description       needle
_exptl_crystal_colour            yellow
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    2.753
_exptl_crystal_F_000             1502
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.351
_exptl_crystal_size_mid          0.073
_exptl_crystal_size_min          0.050
_exptl_absorpt_coefficient_mu    6.806
_shelx_estimated_absorpt_T_min   0.199
_shelx_estimated_absorpt_T_max   0.727
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.199
_exptl_absorpt_correction_T_max  0.727
_exptl_absorpt_process_details   'SADABS (Bruker-AXS, 2004)'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      150(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Apex Duo'
_diffrn_measurement_method       'φ scans'
_diffrn_detector_area_resol_mean 25
_diffrn_reflns_number            13586
_diffrn_reflns_av_unetI/netI     0.0708
_diffrn_reflns_av_R_equivalents  0.0429
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_theta_min         1.639
_diffrn_reflns_theta_max         26.554
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.908
_diffrn_measured_fraction_theta_full 0.916
_diffrn_reflns_Laue_measured_fraction_max 0.908
_diffrn_reflns_Laue_measured_fraction_full 0.916
_diffrn_reflns_point_group_measured_fraction_max 0.908
_diffrn_reflns_point_group_measured_fraction_full 0.916
_reflns_number_total             7405
_reflns_number_gt                5926
_reflns_threshold_expression     >2σ(I)
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_computing_data_collection       'APEX2 (Bruker-AXS, 2004)'
_computing_cell_refinement       'SAINT (Bruker-AXS, 2004)'
_computing_data_reduction        'SAINT (Bruker-AXS, 2004)'
_computing_structure_solution    'SHELXS-2013'
_computing_structure_refinement  'SHELXL-2013'
_computing_molecular_graphics    'SHELXTL (Bruker-AXS, 2004)'
_computing_publication_material  'CIFTAB-97 (Sheldrick, 1998)'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0652P)²+179.1834P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         7405
_refine_ls_number_parameters     415
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.1015
_refine_ls_R_factor_gt           0.0820
_refine_ls_wR_factor_ref         0.2301
_refine_ls_wR_factor_gt          0.2189
_refine_ls_goodness_of_fit_ref   1.128
_refine_ls_restrained_S_all      1.128
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Pt1 Pt 0.13013(7) 0.07773(6) 0.39049(4) 0.01165(19) Uani 1 1 d . . . . .
Nb1 Nb 0.01366(17) 0.28623(14) 0.34189(11) 0.0158(4) Uani 1 1 d . . . . .
Nb2 Nb -0.05047(17) 0.03670(15) 0.20104(11) 0.0178(4) Uani 1 1 d . . . . .
Nb4 Nb -0.30522(17) 0.27574(14) 0.33880(11) 0.0155(4) Uani 1 1 d . . . . .
Nb5 Nb -0.36574(17) 0.04010(15) 0.20643(11) 0.0173(4) Uani 1 1 d . . . . .
Nb6 Nb -0.16946(15) 0.06778(13) 0.40213(10) 0.0103(3) Uani 1 1 d . . . . .
Nb7 Nb -0.18784(18) 0.25154(18) 0.14464(12) 0.0249(4) Uani 1 1 d . . . . .
Cs1 Cs -0.2571(3) -0.0015(3) -0.04739(19) 0.0369(7) Uani 0.5 1 d . . P A .
Cs2 Cs -0.1166(4) 0.5624(3) 0.2623(4) 0.0335(9) Uani 0.4 1 d . . P A 1
Cs3 Cs -0.1147(16) 0.5583(12) 0.3048(11) 0.025(4) Uiso 0.1 1 d . . P A 2
K1 K -0.2319(6) 0.2339(4) 0.6248(3) 0.0349(12) Uani 1 1 d . . . . .
K2 K -0.3580(6) -0.2314(4) 0.3643(4) 0.0367(12) Uani 1 1 d . . . . .
K3 K -0.3072(6) -0.3219(5) -0.0486(4) 0.0475(15) Uani 1 1 d . . . . .
K5 K 0.3699(7) 0.4338(7) 0.3068(6) 0.066(2) Uani 1 1 d . . . . .
K4 K -0.5164(8) 0.0619(9) 0.4253(7) 0.085(3) Uani 1 1 d . . . . .
O16 O 0.0088(12) 0.1748(11) 0.4348(8) 0.016(3) Uani 1 1 d . . . . .
O15 O -0.1527(12) -0.0004(11) 0.5008(8) 0.015(3) Uani 1 1 d . . . . .
O14 O -0.0422(14) -0.0097(11) 0.3313(8) 0.018(3) Uani 1 1 d . . . . .
O13 O -0.2627(12) 0.1824(10) 0.4376(8) 0.013(3) Uani 1 1 d . . . . .
O12 O -0.3151(13) -0.0191(10) 0.3258(8) 0.017(3) Uiso 1 1 d . . . . .
O2P O 0.2901(15) 0.1777(12) 0.4472(10) 0.024(3) Uani 1 1 d . . . . .
O1P O 0.2426(15) -0.0198(12) 0.3342(9) 0.025(3) Uani 1 1 d . . . . .
O11 O -0.5084(15) -0.0500(13) 0.1536(10) 0.027(3) Uani 1 1 d . . . . .
O10 O -0.1715(12) 0.1569(10) 0.2788(8) 0.014(3) Uani 1 1 d . . . . .
O9 O 0.0942(13) 0.1557(11) 0.2817(8) 0.016(3) Uani 1 1 d . . . . .
O8 O -0.1218(14) 0.3534(11) 0.3873(9) 0.021(3) Uani 1 1 d . . . . .
O7 O -0.0254(16) 0.3299(14) 0.2242(12) 0.033(4) Uani 1 1 d . . . . .
O6 O -0.0749(14) 0.1385(14) 0.1169(9) 0.026(3) Uani 1 1 d . . . . .
O5 O 0.0527(14) -0.0531(13) 0.1551(8) 0.023(3) Uani 1 1 d . . . . .
O4 O -0.4001(16) 0.3647(11) 0.3896(10) 0.025(3) Uani 1 1 d . . . . .
O3 O -0.2206(15) -0.0374(11) 0.1676(9) 0.022(3) Uiso 1 1 d . . . . .
O2 O -0.2009(19) 0.3184(18) 0.0485(13) 0.049(5) Uani 1 1 d . . . . .
O1 O 0.1609(15) 0.3702(11) 0.3927(10) 0.024(3) Uani 1 1 d . . . . .
O18 O -0.2825(15) 0.3318(13) 0.2243(10) 0.026(3) Uani 1 1 d . . . . .
O19 O -0.4319(13) 0.1548(11) 0.2760(8) 0.018(3) Uani 1 1 d . . . . .
O17 O -0.3361(14) 0.1344(14) 0.1136(9) 0.028(4) Uani 1 1 d . . . . .
O3W O -0.0712(19) -0.2210(12) 0.3775(9) 0.032(4) Uani 1 1 d . . . . .
O5W O -0.4453(18) -0.1649(16) -0.0038(11) 0.042(5) Uani 1 1 d . . . . .
O6W O -0.3184(18) -0.1972(18) -0.1992(13) 0.048(5) Uani 1 1 d . . . . .
O1W O -0.107(2) 0.4136(12) 0.5733(11) 0.039(4) Uani 1 1 d . . . . .
O8W O -0.1004(18) -0.1693(17) -0.0049(11) 0.046(5) Uani 1 1 d . . . . .
O4W O -0.2845(18) -0.4169(13) 0.4268(12) 0.037(4) Uani 1 1 d . . . . .
O9W O -0.177(2) -0.4422(19) -0.1628(16) 0.062(6) Uani 1 1 d . . . . .
O2W O -0.440(3) 0.372(3) 0.5683(15) 0.061(9) Uani 0.75 1 d . . P . .
O10W O -0.523(3) -0.441(3) -0.157(2) 0.057(8) Uiso 0.7 1 d . . P A .
O11W O -0.470(4) 0.085(3) 0.610(2) 0.061(9) Uiso 0.65 1 d . . P . .
O7W O -0.282(4) -0.260(3) 0.170(2) 0.070(11) Uani 0.7 1 d . . P A .
O12W O -0.494(8) -0.336(6) 0.204(5) 0.08(2) Uiso 0.35 1 d . . P . .
O13W O 0.104(4) 0.744(3) 0.200(2) 0.067(10) Uiso 0.65 1 d . . P . .
O15W O -0.615(5) -0.225(4) 0.226(3) 0.062(13) Uiso 0.45 1 d . . P . .
O16W O 0.061(5) 0.587(4) 0.066(3) 0.052(11) Uiso 0.45 1 d . . P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Pt1 O2P 1.994(14) . ?
Pt1 O15 1.998(11) 2_556 ?
Pt1 O16 2.010(14) . ?
Pt1 O9 2.016(13) . ?
Pt1 O1P 2.019(16) . ?
Pt1 O14 2.029(13) . ?
Pt1 Nb2 3.1414(18) . ?
Pt1 Nb1 3.1432(19) . ?
Pt1 Nb6 3.1720(18) . ?
Pt1 K4 3.709(9) 1_655 ?
Nb1 O1 1.784(15) . ?
Nb1 O7 1.919(16) . ?
Nb1 O8 1.920(15) . ?
Nb1 O16 2.094(13) . ?
Nb1 O9 2.124(14) . ?
Nb1 O10 2.388(12) . ?
Nb1 Nb4 3.335(3) . ?
Nb1 Nb7 3.339(3) . ?
Nb1 Cs3 3.901(16) . ?
Nb1 K5 4.116(8) . ?
Nb1 Cs2 4.126(4) . ?
Nb2 O5 1.817(15) . ?
Nb2 O3 1.885(15) . ?
Nb2 O6 1.913(15) . ?
Nb2 O14 2.106(13) . ?
Nb2 O9 2.134(13) . ?
Nb2 O10 2.418(13) . ?
Nb2 Nb5 3.336(3) . ?
Nb2 Nb7 3.351(3) . ?
Nb2 Cs1 3.992(3) . ?
Nb2 Cs1 4.301(4) 2 ?
Nb4 O4 1.779(16) . ?
Nb4 O19 1.954(13) . ?
Nb4 O18 1.976(14) . ?
Nb4 O13 2.029(12) . ?
Nb4 O8 2.045(14) . ?
Nb4 O10 2.379(13) . ?
Nb4 Nb6 3.297(2) . ?
Nb4 Nb5 3.337(3) . ?
Nb4 Nb7 3.353(3) . ?
Nb4 K4 3.759(9) . ?
Nb4 Cs3 3.998(16) . ?
Nb5 O11 1.793(15) . ?
Nb5 O19 1.957(15) . ?
Nb5 O17 1.971(15) . ?
Nb5 O3 2.035(16) . ?
Nb5 O12 2.047(13) . ?
Nb5 O10 2.407(12) . ?
Nb5 Nb6 3.299(2) . ?
Nb5 K4 3.880(10) . ?
Nb5 Cs1 4.167(3) . ?
Nb5 Cs1 4.258(3) 2_455 ?
Nb6 O15 1.797(11) . ?
Nb6 O12 1.915(13) . ?
Nb6 O13 1.918(13) . ?
Nb6 O14 2.104(14) . ?
Nb6 O16 2.133(13) . ?
Nb6 O10 2.278(12) . ?
Nb6 K4 3.712(9) . ?
Nb6 K1 3.958(6) . ?
Nb6 K2 3.988(6) . ?
Nb7 O2 1.753(15) . ?
Nb7 O18 1.954(17) . ?
Nb7 O17 1.978(15) . ?
Nb7 O7 2.014(17) . ?
Nb7 O6 2.014(17) . ?
Nb7 O10 2.456(13) . ?
Nb7 Cs1 3.996(4) . ?
Nb7 Cs2 4.064(4) . ?
Nb7 Cs3 4.260(16) . ?
Cs1 O5W 2.88(2) . ?
Cs1 O8W 2.90(2) . ?
Cs1 O11 2.913(16) 2_455 ?
Cs1 O5 2.951(13) 2 ?
Cs1 O17 3.103(16) . ?
Cs1 O6W 3.12(2) . ?
Cs1 O6 3.124(15) . ?
Cs1 O3 3.302(14) . ?
Cs1 K3 4.013(8) . ?
Cs2 O3W 3.025(16) 1_565 ?
Cs2 O1W 3.116(19) 2_566 ?
Cs2 O18 3.156(16) . ?
Cs2 O7 3.217(18) . ?
Cs2 O4W 3.27(2) 1_565 ?
Cs2 O7W 3.29(4) 1_565 ?
Cs2 O13W 3.38(4) . ?
Cs2 O8 3.407(14) . ?
Cs2 O16W 3.76(5) . ?
Cs2 K2 4.187(7) 1_565 ?
Cs3 O1W 2.71(3) 2_566 ?
Cs3 O4W 2.78(3) 1_565 ?
Cs3 O3W 2.84(2) 1_565 ?
Cs3 O8 2.99(2) . ?
Cs3 O18 3.19(2) . ?
Cs3 O7 3.31(2) . ?
Cs3 O7W 3.65(4) 1_565 ?
Cs3 O13W 3.74(4) . ?
Cs3 K2 4.030(18) 1_565 ?
Cs3 K1 4.150(17) 2_566 ?
K1 O1W 2.729(17) . ?
K1 O13W 2.76(4) 2_566 ?
K1 O13 2.797(13) . ?
K1 O1P 2.828(16) 2_556 ?
K1 O11W 2.91(4) . ?
K1 O15W 2.97(5) 2_456 ?
K1 O2W 3.04(3) . ?
K1 O3W 3.22(2) 2_556 ?
K1 K4 4.129(12) . ?
K1 Cs3 4.150(17) 2_566 ?
K1 Cs2 4.225(7) 2_566 ?
K2 O12W 2.73(8) . ?
K2 O4W 2.767(17) . ?
K2 O11W 2.78(4) 2_456 ?
K2 O12 2.800(14) . ?
K2 O2P 2.819(15) 2_556 ?
K2 O2W 2.97(3) 2_456 ?
K2 O3W 2.98(2) . ?
K2 O7W 3.15(4) . ?
K2 O15W 3.17(5) . ?
K2 Cs3 4.030(18) 1_545 ?
K2 K4 4.118(13) 2_456 ?
K3 O8W 2.676(19) . ?
K3 O5W 2.68(2) . ?
K3 O10W 2.76(3) . ?
K3 O9W 2.80(3) . ?
K3 O6W 2.899(18) . ?
K3 O7W 3.28(3) . ?
K3 K5 3.935(11) 2 ?
K3 Cs2 5.248(8) 1_545 ?
K5 O9W 2.76(3) 2 ?
K5 O1 2.800(17) . ?
K5 O4 2.828(18) 1_655 ?
K5 O2W 2.88(3) 2_566 ?
K5 O10W 2.97(3) 2 ?
K5 O6W 3.19(3) 2 ?
K5 K3 3.935(11) 2 ?
K5 Nb4 4.152(8) 1_655 ?
K5 K1 4.665(11) 2_566 ?
K5 K2 4.727(10) 1_665 ?
K4 O11W 1.85(4) 2_456 ?
K4 O2P 2.685(19) 1_455 ?
K4 O1P 2.719(18) 1_455 ?
K4 O11W 2.73(4) . ?
K4 O19 2.861(15) . ?
K4 O13 2.877(15) . ?
K4 K4 2.883(18) 2_456 ?
K4 O12 2.993(17) . ?
K4 Pt1 3.709(9) 1_455 ?
O15 Pt1 1.997(11) 2_556 ?
O2P K4 2.685(19) 1_655 ?
O2P K2 2.819(15) 2_556 ?
O1P K4 2.719(18) 1_655 ?
O1P K1 2.828(16) 2_556 ?
O11 Cs1 2.913(16) 2_455 ?
O5 Cs1 2.951(13) 2 ?
O4 K5 2.828(18) 1_455 ?
O3W Cs3 2.84(2) 1_545 ?
O3W Cs2 3.025(16) 1_545 ?
O3W K1 3.22(2) 2_556 ?
O6W K5 3.19(3) 2 ?
O1W Cs3 2.71(3) 2_566 ?
O1W Cs2 3.116(19) 2_566 ?
O4W Cs3 2.78(3) 1_545 ?
O4W Cs2 3.27(2) 1_545 ?
O9W K5 2.76(3) 2 ?
O2W K5 2.88(3) 2_566 ?
O2W K2 2.97(3) 2_456 ?
O10W K5 2.97(3) 2 ?
O11W K4 1.85(4) 2_456 ?
O11W K2 2.78(4) 2_456 ?
O7W Cs2 3.29(4) 1_545 ?
O7W Cs3 3.65(4) 1_545 ?
O13W K1 2.76(4) 2_566 ?
O15W K1 2.97(5) 2_456 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2P Pt1 O15 87.8(5) . 2_556 ?
O2P Pt1 O16 94.2(6) . . ?
O15 Pt1 O16 96.2(5) 2_556 . ?
O2P Pt1 O9 94.9(5) . . ?
O15 Pt1 O9 176.0(5) 2_556 . ?
O16 Pt1 O9 80.7(5) . . ?
O2P Pt1 O1P 89.0(6) . . ?
O15 Pt1 O1P 88.3(6) 2_556 . ?
O16 Pt1 O1P 174.6(5) . . ?
O9 Pt1 O1P 94.7(6) . . ?
O2P Pt1 O14 173.8(6) . . ?
O15 Pt1 O14 95.9(5) 2_556 . ?
O16 Pt1 O14 80.6(5) . . ?
O9 Pt1 O14 81.1(5) . . ?
O1P Pt1 O14 96.0(6) . . ?
O2P Pt1 Nb2 135.8(4) . . ?
O15 Pt1 Nb2 135.7(4) 2_556 . ?
O16 Pt1 Nb2 88.9(4) . . ?
O9 Pt1 Nb2 42.2(4) . . ?
O1P Pt1 Nb2 85.8(4) . . ?
O14 Pt1 Nb2 41.5(4) . . ?
O2P Pt1 Nb1 85.5(4) . . ?
O15 Pt1 Nb1 135.7(4) 2_556 . ?
O16 Pt1 Nb1 41.0(4) . . ?
O9 Pt1 Nb1 41.9(4) . . ?
O1P Pt1 Nb1 135.2(4) . . ?
O14 Pt1 Nb1 88.4(4) . . ?
Nb2 Pt1 Nb1 68.54(5) . . ?
O2P Pt1 Nb6 134.8(5) . . ?
O15 Pt1 Nb6 88.9(4) 2_556 . ?
O16 Pt1 Nb6 41.5(4) . . ?
O9 Pt1 Nb6 87.1(4) . . ?
O1P Pt1 Nb6 136.0(4) . . ?
O14 Pt1 Nb6 40.7(4) . . ?
Nb2 Pt1 Nb6 66.54(4) . . ?
Nb1 Pt1 Nb6 66.33(4) . . ?
O2P Pt1 K4 44.7(5) . 1_655 ?
O15 Pt1 K4 78.2(4) 2_556 1_655 ?
O16 Pt1 K4 138.1(4) . 1_655 ?
O9 Pt1 K4 105.9(4) . 1_655 ?
O1P Pt1 K4 45.8(5) . 1_655 ?
O14 Pt1 K4 141.0(4) . 1_655 ?
Nb2 Pt1 K4 124.13(17) . 1_655 ?
Nb1 Pt1 K4 122.85(16) . 1_655 ?
Nb6 Pt1 K4 166.99(14) . 1_655 ?
O1 Nb1 O7 104.3(7) . . ?
O1 Nb1 O8 105.3(6) . . ?
O7 Nb1 O8 94.0(7) . . ?
O1 Nb1 O16 99.1(6) . . ?
O7 Nb1 O16 153.6(6) . . ?
O8 Nb1 O16 91.5(6) . . ?
O1 Nb1 O9 98.8(6) . . ?
O7 Nb1 O9 88.0(6) . . ?
O8 Nb1 O9 154.5(6) . . ?
O16 Nb1 O9 76.3(5) . . ?
O1 Nb1 O10 173.5(6) . . ?
O7 Nb1 O10 79.9(6) . . ?
O8 Nb1 O10 79.2(5) . . ?
O16 Nb1 O10 75.8(5) . . ?
O9 Nb1 O10 76.2(5) . . ?
O1 Nb1 Pt1 91.8(5) . . ?
O7 Nb1 Pt1 127.1(6) . . ?
O8 Nb1 Pt1 130.1(4) . . ?
O16 Nb1 Pt1 39.0(4) . . ?
O9 Nb1 Pt1 39.3(3) . . ?
O10 Nb1 Pt1 81.7(3) . . ?
O1 Nb1 Nb4 139.2(5) . . ?
O7 Nb1 Nb4 84.0(5) . . ?
O8 Nb1 Nb4 33.9(4) . . ?
O16 Nb1 Nb4 86.3(4) . . ?
O9 Nb1 Nb4 121.6(4) . . ?
O10 Nb1 Nb4 45.5(3) . . ?
Pt1 Nb1 Nb4 115.17(6) . . ?
O1 Nb1 Nb7 137.1(5) . . ?
O7 Nb1 Nb7 32.8(5) . . ?
O8 Nb1 Nb7 84.5(4) . . ?
O16 Nb1 Nb7 122.7(4) . . ?
O9 Nb1 Nb7 83.6(3) . . ?
O10 Nb1 Nb7 47.3(3) . . ?
Pt1 Nb1 Nb7 113.91(7) . . ?
Nb4 Nb1 Nb7 60.33(5) . . ?
O1 Nb1 Cs3 84.1(5) . . ?
O7 Nb1 Cs3 57.8(6) . . ?
O8 Nb1 Cs3 48.2(5) . . ?
O16 Nb1 Cs3 138.0(5) . . ?
O9 Nb1 Cs3 145.0(4) . . ?
O10 Nb1 Cs3 102.4(4) . . ?
Pt1 Nb1 Cs3 174.4(3) . . ?
Nb4 Nb1 Cs3 66.5(2) . . ?
Nb7 Nb1 Cs3 71.6(2) . . ?
O1 Nb1 K5 33.2(5) . . ?
O7 Nb1 K5 78.0(5) . . ?
O8 Nb1 K5 127.3(4) . . ?
O16 Nb1 K5 118.3(4) . . ?
O9 Nb1 K5 78.0(4) . . ?
O10 Nb1 K5 146.3(3) . . ?
Pt1 Nb1 K5 91.78(13) . . ?
Nb4 Nb1 K5 153.01(14) . . ?
Nb7 Nb1 K5 108.69(13) . . ?
Cs3 Nb1 K5 86.8(3) . . ?
O1 Nb1 Cs2 86.4(5) . . ?
O7 Nb1 Cs2 49.2(6) . . ?
O8 Nb1 Cs2 54.9(4) . . ?
O16 Nb1 Cs2 145.9(4) . . ?
O9 Nb1 Cs2 136.4(4) . . ?
O10 Nb1 Cs2 100.1(3) . . ?
Pt1 Nb1 Cs2 174.95(9) . . ?
Nb4 Nb1 Cs2 68.90(7) . . ?
Nb7 Nb1 Cs2 64.97(8) . . ?
K5 Nb1 Cs2 84.10(14) . . ?
O5 Nb2 O3 105.1(6) . . ?
O5 Nb2 O6 105.5(6) . . ?
O3 Nb2 O6 94.4(6) . . ?
O5 Nb2 O14 99.7(6) . . ?
O3 Nb2 O14 90.1(6) . . ?
O6 Nb2 O14 152.2(6) . . ?
O5 Nb2 O9 99.9(6) . . ?
O3 Nb2 O9 153.4(6) . . ?
O6 Nb2 O9 87.5(6) . . ?
O14 Nb2 O9 76.7(5) . . ?
O5 Nb2 O10 173.4(5) . . ?
O3 Nb2 O10 79.0(5) . . ?
O6 Nb2 O10 79.2(6) . . ?
O14 Nb2 O10 74.8(5) . . ?
O9 Nb2 O10 75.4(5) . . ?
O5 Nb2 Pt1 92.1(4) . . ?
O3 Nb2 Pt1 129.4(4) . . ?
O6 Nb2 Pt1 126.6(5) . . ?
O14 Nb2 Pt1 39.7(4) . . ?
O9 Nb2 Pt1 39.4(3) . . ?
O10 Nb2 Pt1 81.3(3) . . ?
O5 Nb2 Nb5 138.1(4) . . ?
O3 Nb2 Nb5 33.1(5) . . ?
O6 Nb2 Nb5 84.0(4) . . ?
O14 Nb2 Nb5 85.0(4) . . ?
O9 Nb2 Nb5 121.4(4) . . ?
O10 Nb2 Nb5 46.1(3) . . ?
Pt1 Nb2 Nb5 115.06(6) . . ?
O5 Nb2 Nb7 137.8(4) . . ?
O3 Nb2 Nb7 84.4(5) . . ?
O6 Nb2 Nb7 32.4(5) . . ?
O14 Nb2 Nb7 121.6(4) . . ?
O9 Nb2 Nb7 83.2(4) . . ?
O10 Nb2 Nb7 47.0(3) . . ?
Pt1 Nb2 Nb7 113.62(7) . . ?
Nb5 Nb2 Nb7 60.55(6) . . ?
O5 Nb2 Cs1 86.3(4) . . ?
O3 Nb2 Cs1 55.2(4) . . ?
O6 Nb2 Cs1 49.9(5) . . ?
O14 Nb2 Cs1 144.9(4) . . ?
O9 Nb2 Cs1 136.6(4) . . ?
O10 Nb2 Cs1 100.3(3) . . ?
Pt1 Nb2 Cs1 175.35(7) . . ?
Nb5 Nb2 Cs1 68.65(6) . . ?
Nb7 Nb2 Cs1 65.27(7) . . ?
O5 Nb2 Cs1 33.1(5) . 2 ?
O3 Nb2 Cs1 124.4(4) . 2 ?
O6 Nb2 Cs1 77.1(5) . 2 ?
O14 Nb2 Cs1 122.0(4) . 2 ?
O9 Nb2 Cs1 81.9(4) . 2 ?
O10 Nb2 Cs1 147.7(3) . 2 ?
Pt1 Nb2 Cs1 95.58(6) . 2 ?
Nb5 Nb2 Cs1 149.35(7) . 2 ?
Nb7 Nb2 Cs1 108.17(7) . 2 ?
Cs1 Nb2 Cs1 80.74(7) . 2 ?
O4 Nb4 O19 104.4(7) . . ?
O4 Nb4 O18 104.2(7) . . ?
O19 Nb4 O18 91.9(6) . . ?
O4 Nb4 O13 101.7(6) . . ?
O19 Nb4 O13 87.5(5) . . ?
O18 Nb4 O13 153.4(6) . . ?
O4 Nb4 O8 100.9(7) . . ?
O19 Nb4 O8 154.4(6) . . ?
O18 Nb4 O8 85.7(6) . . ?
O13 Nb4 O8 83.5(5) . . ?
O4 Nb4 O10 176.9(6) . . ?
O19 Nb4 O10 77.4(5) . . ?
O18 Nb4 O10 78.1(6) . . ?
O13 Nb4 O10 75.8(5) . . ?
O8 Nb4 O10 77.1(5) . . ?
O4 Nb4 Nb6 133.9(5) . . ?
O19 Nb4 Nb6 78.1(4) . . ?
O18 Nb4 Nb6 121.8(5) . . ?
O13 Nb4 Nb6 32.3(4) . . ?
O8 Nb4 Nb6 81.5(4) . . ?
O10 Nb4 Nb6 43.7(3) . . ?
O4 Nb4 Nb1 132.4(5) . . ?
O19 Nb4 Nb1 123.1(4) . . ?
O18 Nb4 Nb1 77.4(4) . . ?
O13 Nb4 Nb1 80.7(4) . . ?
O8 Nb4 Nb1 31.6(4) . . ?
O10 Nb4 Nb1 45.7(3) . . ?
Nb6 Nb4 Nb1 62.80(5) . . ?
O4 Nb4 Nb5 135.8(5) . . ?
O19 Nb4 Nb5 31.5(4) . . ?
O18 Nb4 Nb5 82.6(5) . . ?
O13 Nb4 Nb5 83.2(4) . . ?
O8 Nb4 Nb5 123.2(4) . . ?
O10 Nb4 Nb5 46.1(3) . . ?
Nb6 Nb4 Nb5 59.63(5) . . ?
Nb1 Nb4 Nb5 91.74(6) . . ?
O4 Nb4 Nb7 135.4(5) . . ?
O19 Nb4 Nb7 82.5(4) . . ?
O18 Nb4 Nb7 31.2(5) . . ?
O13 Nb4 Nb7 122.8(4) . . ?
O8 Nb4 Nb7 82.3(4) . . ?
O10 Nb4 Nb7 47.0(3) . . ?
Nb6 Nb4 Nb7 90.70(6) . . ?
Nb1 Nb4 Nb7 59.89(5) . . ?
Nb5 Nb4 Nb7 60.50(6) . . ?
O4 Nb4 K4 84.1(5) . . ?
O19 Nb4 K4 48.4(4) . . ?
O18 Nb4 K4 139.8(5) . . ?
O13 Nb4 K4 49.2(4) . . ?
O8 Nb4 K4 132.0(4) . . ?
O10 Nb4 K4 95.5(3) . . ?
Nb6 Nb4 K4 63.10(15) . . ?
Nb1 Nb4 K4 125.53(16) . . ?
Nb5 Nb4 K4 65.98(19) . . ?
Nb7 Nb4 K4 126.45(19) . . ?
O4 Nb4 Cs3 80.1(5) . . ?
O19 Nb4 Cs3 142.8(4) . . ?
O18 Nb4 Cs3 52.0(5) . . ?
O13 Nb4 Cs3 128.4(4) . . ?
O8 Nb4 Cs3 46.5(5) . . ?
O10 Nb4 Cs3 100.0(4) . . ?
Nb6 Nb4 Cs3 125.5(2) . . ?
Nb1 Nb4 Cs3 63.5(2) . . ?
Nb5 Nb4 Cs3 130.7(2) . . ?
Nb7 Nb4 Cs3 70.2(2) . . ?
K4 Nb4 Cs3 162.9(3) . . ?
O11 Nb5 O19 104.3(6) . . ?
O11 Nb5 O17 103.0(6) . . ?
O19 Nb5 O17 90.6(6) . . ?
O11 Nb5 O3 102.4(6) . . ?
O19 Nb5 O3 153.1(6) . . ?
O17 Nb5 O3 86.6(6) . . ?
O11 Nb5 O12 102.9(6) . . ?
O19 Nb5 O12 87.1(5) . . ?
O17 Nb5 O12 153.7(6) . . ?
O3 Nb5 O12 83.7(6) . . ?
O11 Nb5 O10 178.4(6) . . ?
O19 Nb5 O10 76.7(5) . . ?
O17 Nb5 O10 78.1(5) . . ?
O3 Nb5 O10 76.5(5) . . ?
O12 Nb5 O10 75.9(5) . . ?
O11 Nb5 Nb6 135.2(5) . . ?
O19 Nb5 Nb6 78.0(4) . . ?
O17 Nb5 Nb6 121.8(4) . . ?
O3 Nb5 Nb6 80.7(4) . . ?
O12 Nb5 Nb6 32.4(4) . . ?
O10 Nb5 Nb6 43.7(3) . . ?
O11 Nb5 Nb2 132.6(5) . . ?
O19 Nb5 Nb2 123.1(4) . . ?
O17 Nb5 Nb2 78.2(5) . . ?
O3 Nb5 Nb2 30.4(4) . . ?
O12 Nb5 Nb2 81.2(4) . . ?
O10 Nb5 Nb2 46.4(3) . . ?
Nb6 Nb5 Nb2 62.93(5) . . ?
O11 Nb5 Nb4 135.7(5) . . ?
O19 Nb5 Nb4 31.4(4) . . ?
O17 Nb5 Nb4 81.6(5) . . ?
O3 Nb5 Nb4 122.0(4) . . ?
O12 Nb5 Nb4 82.9(4) . . ?
O10 Nb5 Nb4 45.4(3) . . ?
Nb6 Nb5 Nb4 59.57(5) . . ?
Nb2 Nb5 Nb4 91.72(6) . . ?
O11 Nb5 K4 88.0(5) . . ?
O19 Nb5 K4 45.2(4) . . ?
O17 Nb5 K4 135.7(5) . . ?
O3 Nb5 K4 133.3(4) . . ?
O12 Nb5 K4 49.7(4) . . ?
O10 Nb5 K4 92.0(3) . . ?
Nb6 Nb5 K4 61.65(14) . . ?
Nb2 Nb5 K4 124.53(15) . . ?
Nb4 Nb5 K4 62.23(17) . . ?
O11 Nb5 Cs1 84.2(5) . . ?
O19 Nb5 Cs1 135.1(4) . . ?
O17 Nb5 Cs1 45.0(5) . . ?
O3 Nb5 Cs1 51.3(4) . . ?
O12 Nb5 Cs1 134.7(4) . . ?
O10 Nb5 Cs1 95.9(3) . . ?
Nb6 Nb5 Cs1 126.08(7) . . ?
Nb2 Nb5 Cs1 63.15(6) . . ?
Nb4 Nb5 Cs1 122.77(7) . . ?
K4 Nb5 Cs1 171.83(16) . . ?
O11 Nb5 Cs1 32.6(5) . 2_455 ?
O19 Nb5 Cs1 83.2(4) . 2_455 ?
O17 Nb5 Cs1 78.7(4) . 2_455 ?
O3 Nb5 Cs1 122.2(4) . 2_455 ?
O12 Nb5 Cs1 126.8(4) . 2_455 ?
O10 Nb5 Cs1 149.0(3) . 2_455 ?
Nb6 Nb5 Cs1 151.94(7) . 2_455 ?
Nb2 Nb5 Cs1 144.86(7) . 2_455 ?
Nb4 Nb5 Cs1 110.67(7) . 2_455 ?
K4 Nb5 Cs1 90.34(15) . 2_455 ?
Cs1 Nb5 Cs1 81.81(7) . 2_455 ?
O15 Nb6 O12 102.4(6) . . ?
O15 Nb6 O13 102.1(6) . . ?
O12 Nb6 O13 95.8(6) . . ?
O15 Nb6 O14 98.9(6) . . ?
O12 Nb6 O14 90.1(5) . . ?
O13 Nb6 O14 156.5(5) . . ?
O15 Nb6 O16 98.1(5) . . ?
O12 Nb6 O16 156.9(5) . . ?
O13 Nb6 O16 90.3(5) . . ?
O14 Nb6 O16 76.1(5) . . ?
O15 Nb6 O10 175.0(5) . . ?
O12 Nb6 O10 81.6(5) . . ?
O13 Nb6 O10 80.4(5) . . ?
O14 Nb6 O10 78.0(5) . . ?
O16 Nb6 O10 77.5(5) . . ?
O15 Nb6 Pt1 92.4(4) . . ?
O12 Nb6 Pt1 128.9(4) . . ?
O13 Nb6 Pt1 128.7(4) . . ?
O14 Nb6 Pt1 39.0(4) . . ?
O16 Nb6 Pt1 38.6(4) . . ?
O10 Nb6 Pt1 82.7(3) . . ?
O15 Nb6 Nb4 136.5(4) . . ?
O12 Nb6 Nb4 85.9(4) . . ?
O13 Nb6 Nb4 34.5(4) . . ?
O14 Nb6 Nb4 124.0(4) . . ?
O16 Nb6 Nb4 86.6(4) . . ?
O10 Nb6 Nb4 46.2(3) . . ?
Pt1 Nb6 Nb4 115.45(6) . . ?
O15 Nb6 Nb5 137.3(4) . . ?
O12 Nb6 Nb5 34.9(4) . . ?
O13 Nb6 Nb5 85.9(4) . . ?
O14 Nb6 Nb5 86.0(3) . . ?
O16 Nb6 Nb5 124.1(3) . . ?
O10 Nb6 Nb5 46.9(3) . . ?
Pt1 Nb6 Nb5 115.26(6) . . ?
Nb4 Nb6 Nb5 60.80(5) . . ?
O15 Nb6 K4 86.3(4) . . ?
O12 Nb6 K4 53.3(5) . . ?
O13 Nb6 K4 49.9(4) . . ?
O14 Nb6 K4 143.1(4) . . ?
O16 Nb6 K4 139.6(4) . . ?
O10 Nb6 K4 98.6(4) . . ?
Pt1 Nb6 K4 177.66(19) . . ?
Nb4 Nb6 K4 64.54(16) . . ?
Nb5 Nb6 K4 66.90(17) . . ?
O15 Nb6 K1 64.8(5) . . ?
O12 Nb6 K1 118.0(4) . . ?
O13 Nb6 K1 40.6(4) . . ?
O14 Nb6 K1 149.3(4) . . ?
O16 Nb6 K1 80.6(4) . . ?
O10 Nb6 K1 116.2(3) . . ?
Pt1 Nb6 K1 112.64(9) . . ?
Nb4 Nb6 K1 73.56(9) . . ?
Nb5 Nb6 K1 123.96(10) . . ?
K4 Nb6 K1 65.0(2) . . ?
O15 Nb6 K2 65.8(4) . . ?
O12 Nb6 K2 39.8(4) . . ?
O13 Nb6 K2 117.6(4) . . ?
O14 Nb6 K2 80.9(4) . . ?
O16 Nb6 K2 149.5(4) . . ?
O10 Nb6 K2 117.0(3) . . ?
Pt1 Nb6 K2 113.31(10) . . ?
Nb4 Nb6 K2 123.15(10) . . ?
Nb5 Nb6 K2 73.24(9) . . ?
K4 Nb6 K2 67.9(2) . . ?
K1 Nb6 K2 111.89(12) . . ?
O2 Nb7 O18 103.3(8) . . ?
O2 Nb7 O17 102.7(8) . . ?
O18 Nb7 O17 90.6(7) . . ?
O2 Nb7 O7 104.0(8) . . ?
O18 Nb7 O7 86.1(7) . . ?
O17 Nb7 O7 153.1(6) . . ?
O2 Nb7 O6 103.6(8) . . ?
O18 Nb7 O6 152.9(6) . . ?
O17 Nb7 O6 86.5(7) . . ?
O7 Nb7 O6 84.5(7) . . ?
O2 Nb7 O10 179.5(8) . . ?
O18 Nb7 O10 76.6(5) . . ?
O17 Nb7 O10 76.8(5) . . ?
O7 Nb7 O10 76.5(5) . . ?
O6 Nb7 O10 76.5(5) . . ?
O2 Nb7 Nb1 134.9(7) . . ?
O18 Nb7 Nb1 77.6(4) . . ?
O17 Nb7 Nb1 122.4(4) . . ?
O7 Nb7 Nb1 31.1(4) . . ?
O6 Nb7 Nb1 81.3(4) . . ?
O10 Nb7 Nb1 45.6(3) . . ?
O2 Nb7 Nb2 134.0(7) . . ?
O18 Nb7 Nb2 122.7(4) . . ?
O17 Nb7 Nb2 77.8(5) . . ?
O7 Nb7 Nb2 81.7(5) . . ?
O6 Nb7 Nb2 30.6(4) . . ?
O10 Nb7 Nb2 46.1(3) . . ?
Nb1 Nb7 Nb2 63.88(5) . . ?
O2 Nb7 Nb4 134.8(7) . . ?
O18 Nb7 Nb4 31.6(4) . . ?
O17 Nb7 Nb4 81.1(4) . . ?
O7 Nb7 Nb4 82.2(5) . . ?
O6 Nb7 Nb4 121.6(4) . . ?
O10 Nb7 Nb4 45.1(3) . . ?
Nb1 Nb7 Nb4 59.77(5) . . ?
Nb2 Nb7 Nb4 91.17(6) . . ?
O2 Nb7 Cs1 80.2(8) . . ?
O18 Nb7 Cs1 138.9(5) . . ?
O17 Nb7 Cs1 49.6(5) . . ?
O7 Nb7 Cs1 133.5(5) . . ?
O6 Nb7 Cs1 50.4(4) . . ?
O10 Nb7 Cs1 99.5(3) . . ?
Nb1 Nb7 Cs1 128.60(8) . . ?
Nb2 Nb7 Cs1 65.13(7) . . ?
Nb4 Nb7 Cs1 127.57(8) . . ?
O2 Nb7 Cs2 79.8(8) . . ?
O18 Nb7 Cs2 49.2(4) . . ?
O17 Nb7 Cs2 138.0(5) . . ?
O7 Nb7 Cs2 51.4(5) . . ?
O6 Nb7 Cs2 134.3(4) . . ?
O10 Nb7 Cs2 100.5(3) . . ?
Nb1 Nb7 Cs2 66.92(8) . . ?
Nb2 Nb7 Cs2 130.31(9) . . ?
Nb4 Nb7 Cs2 69.56(9) . . ?
Cs1 Nb7 Cs2 159.92(10) . . ?
O2 Nb7 Cs3 88.2(8) . . ?
O18 Nb7 Cs3 44.8(5) . . ?
O17 Nb7 Cs3 135.3(5) . . ?
O7 Nb7 Cs3 48.9(6) . . ?
O6 Nb7 Cs3 133.4(5) . . ?
O10 Nb7 Cs3 92.1(4) . . ?
Nb1 Nb7 Cs3 60.3(2) . . ?
Nb2 Nb7 Cs3 124.2(2) . . ?
Nb4 Nb7 Cs3 62.0(2) . . ?
Cs1 Nb7 Cs3 168.4(2) . . ?
O5W Cs1 O8W 77.9(5) . . ?
O5W Cs1 O11 80.5(4) . 2_455 ?
O8W Cs1 O11 145.8(5) . 2_455 ?
O5W Cs1 O5 147.4(5) . 2 ?
O8W Cs1 O5 81.7(5) . 2 ?
O11 Cs1 O5 103.9(4) 2_455 2 ?
O5W Cs1 O17 82.6(5) . . ?
O8W Cs1 O17 117.0(4) . . ?
O11 Cs1 O17 85.8(4) 2_455 . ?
O5 Cs1 O17 129.6(4) 2 . ?
O5W Cs1 O6W 69.5(5) . . ?
O8W Cs1 O6W 68.5(5) . . ?
O11 Cs1 O6W 79.2(5) 2_455 . ?
O5 Cs1 O6W 79.5(4) 2 . ?
O17 Cs1 O6W 150.1(4) . . ?
O5W Cs1 O6 115.8(4) . . ?
O8W Cs1 O6 85.1(5) . . ?
O11 Cs1 O6 128.5(4) 2_455 . ?
O5 Cs1 O6 87.1(4) 2 . ?
O17 Cs1 O6 52.1(4) . . ?
O6W Cs1 O6 151.7(5) . . ?
O5W Cs1 O3 65.2(4) . . ?
O8W Cs1 O3 66.8(4) . . ?
O11 Cs1 O3 125.7(4) 2_455 . ?
O5 Cs1 O3 127.9(4) 2 . ?
O17 Cs1 O3 50.7(4) . . ?
O6W Cs1 O3 121.0(4) . . ?
O6 Cs1 O3 51.3(4) . . ?
O5W Cs1 Nb2 92.3(3) . . ?
O8W Cs1 Nb2 63.9(3) . . ?
O11 Cs1 Nb2 143.4(3) 2_455 . ?
O5 Cs1 Nb2 101.3(3) 2 . ?
O17 Cs1 Nb2 57.7(3) . . ?
O6W Cs1 Nb2 131.7(3) . . ?
O6 Cs1 Nb2 27.9(3) . . ?
O3 Cs1 Nb2 28.0(3) . . ?
O5W Cs1 Nb7 110.1(4) . . ?
O8W Cs1 Nb7 112.9(3) . . ?
O11 Cs1 Nb7 99.3(3) 2_455 . ?
O5 Cs1 Nb7 101.1(3) 2 . ?
O17 Cs1 Nb7 29.0(3) . . ?
O6W Cs1 Nb7 178.5(4) . . ?
O6 Cs1 Nb7 29.8(3) . . ?
O3 Cs1 Nb7 59.7(3) . . ?
Nb2 Cs1 Nb7 49.60(5) . . ?
O5W Cs1 K3 41.9(4) . . ?
O8W Cs1 K3 41.8(4) . . ?
O11 Cs1 K3 106.3(3) 2_455 . ?
O5 Cs1 K3 107.8(3) 2 . ?
O17 Cs1 K3 116.7(3) . . ?
O6W Cs1 K3 45.9(3) . . ?
O6 Cs1 K3 117.9(3) . . ?
O3 Cs1 K3 75.1(3) . . ?
Nb2 Cs1 K3 90.51(12) . . ?
Nb7 Cs1 K3 134.79(13) . . ?
O5W Cs1 Nb5 62.0(3) . . ?
O8W Cs1 Nb5 94.5(3) . . ?
O11 Cs1 Nb5 98.4(3) 2_455 . ?
O5 Cs1 Nb5 145.4(3) 2 . ?
O17 Cs1 Nb5 26.7(3) . . ?
O6W Cs1 Nb5 131.1(3) . . ?
O6 Cs1 Nb5 58.3(3) . . ?
O3 Cs1 Nb5 28.8(3) . . ?
Nb2 Cs1 Nb5 48.20(5) . . ?
Nb7 Cs1 Nb5 48.72(5) . . ?
K3 Cs1 Nb5 90.51(12) . . ?
O3W Cs2 O1W 65.5(5) 1_565 2_566 ?
O3W Cs2 O18 145.1(5) 1_565 . ?
O1W Cs2 O18 113.2(4) 2_566 . ?
O3W Cs2 O7 147.6(5) 1_565 . ?
O1W Cs2 O7 82.1(4) 2_566 . ?
O18 Cs2 O7 50.3(4) . . ?
O3W Cs2 O4W 64.3(4) 1_565 1_565 ?
O1W Cs2 O4W 80.3(5) 2_566 1_565 ?
O18 Cs2 O4W 80.9(4) . 1_565 ?
O7 Cs2 O4W 114.0(4) . 1_565 ?
O3W Cs2 O7W 67.1(6) 1_565 1_565 ?
O1W Cs2 O7W 131.8(6) 2_566 1_565 ?
O18 Cs2 O7W 110.6(6) . 1_565 ?
O7 Cs2 O7W 143.9(6) . 1_565 ?
O4W Cs2 O7W 87.6(8) 1_565 1_565 ?
O3W Cs2 O13W 66.1(7) 1_565 . ?
O1W Cs2 O13W 79.3(7) 2_566 . ?
O18 Cs2 O13W 148.6(7) . . ?
O7 Cs2 O13W 107.3(8) . . ?
O4W Cs2 O13W 130.4(7) 1_565 . ?
O7W Cs2 O13W 73.8(10) 1_565 . ?
O3W Cs2 O8 112.6(4) 1_565 . ?
O1W Cs2 O8 64.9(4) 2_566 . ?
O18 Cs2 O8 49.1(4) . . ?
O7 Cs2 O8 50.1(4) . . ?
O4W Cs2 O8 64.9(4) 1_565 . ?
O7W Cs2 O8 146.4(8) 1_565 . ?
O13W Cs2 O8 138.6(7) . . ?
O3W Cs2 O16W 108.0(8) 1_565 . ?
O1W Cs2 O16W 103.2(8) 2_566 . ?
O18 Cs2 O16W 106.1(8) . . ?
O7 Cs2 O16W 76.2(8) . . ?
O4W Cs2 O16W 169.7(8) 1_565 . ?
O7W Cs2 O16W 82.9(11) 1_565 . ?
O13W Cs2 O16W 42.6(10) . . ?
O8 Cs2 O16W 125.4(8) . . ?
O3W Cs2 Nb7 170.7(3) 1_565 . ?
O1W Cs2 Nb7 109.4(3) 2_566 . ?
O18 Cs2 Nb7 28.0(3) . . ?
O7 Cs2 Nb7 29.3(3) . . ?
O4W Cs2 Nb7 107.7(3) 1_565 . ?
O7W Cs2 Nb7 118.7(5) 1_565 . ?
O13W Cs2 Nb7 121.6(7) . . ?
O8 Cs2 Nb7 58.4(3) . . ?
O16W Cs2 Nb7 80.4(7) . . ?
O3W Cs2 Nb1 125.1(3) 1_565 . ?
O1W Cs2 Nb1 62.0(3) 2_566 . ?
O18 Cs2 Nb1 55.3(3) . . ?
O7 Cs2 Nb1 26.8(3) . . ?
O4W Cs2 Nb1 91.8(3) 1_565 . ?
O7W Cs2 Nb1 165.7(5) 1_565 . ?
O13W Cs2 Nb1 116.6(7) . . ?
O8 Cs2 Nb1 27.5(3) . . ?
O16W Cs2 Nb1 98.4(8) . . ?
Nb7 Cs2 Nb1 48.11(6) . . ?
O3W Cs2 K2 45.3(4) 1_565 1_565 ?
O1W Cs2 K2 100.3(4) 2_566 1_565 ?
O18 Cs2 K2 105.5(3) . 1_565 ?
O7 Cs2 K2 152.6(3) . 1_565 ?
O4W Cs2 K2 41.3(3) 1_565 1_565 ?
O7W Cs2 K2 48.1(7) 1_565 1_565 ?
O13W Cs2 K2 99.9(7) . 1_565 ?
O8 Cs2 K2 106.0(3) . 1_565 ?
O16W Cs2 K2 128.5(8) . 1_565 ?
Nb7 Cs2 K2 132.00(13) . 1_565 ?
Nb1 Cs2 K2 133.10(16) . 1_565 ?
O1W Cs3 O4W 97.4(8) 2_566 1_565 ?
O1W Cs3 O3W 73.6(6) 2_566 1_565 ?
O4W Cs3 O3W 73.4(6) 1_565 1_565 ?
O1W Cs3 O8 75.9(6) 2_566 . ?
O4W Cs3 O8 76.8(6) 1_565 . ?
O3W Cs3 O8 133.6(7) 1_565 . ?
O1W Cs3 O18 125.2(7) 2_566 . ?
O4W Cs3 O18 88.5(6) 1_565 . ?
O3W Cs3 O18 156.2(8) 1_565 . ?
O8 Cs3 O18 52.5(5) . . ?
O1W Cs3 O7 86.9(6) 2_566 . ?
O4W Cs3 O7 126.6(7) 1_565 . ?
O3W Cs3 O7 154.4(8) 1_565 . ?
O8 Cs3 O7 52.7(5) . . ?
O18 Cs3 O7 49.3(5) . . ?
O1W Cs3 O7W 133.1(8) 2_566 1_565 ?
O4W Cs3 O7W 88.7(9) 1_565 1_565 ?
O3W Cs3 O7W 63.8(6) 1_565 1_565 ?
O8 Cs3 O7W 149.6(8) . 1_565 ?
O18 Cs3 O7W 101.3(7) . 1_565 ?
O7 Cs3 O7W 125.5(8) . 1_565 ?
O1W Cs3 O13W 78.4(8) 2_566 . ?
O4W Cs3 O13W 135.4(9) 1_565 . ?
O3W Cs3 O13W 62.7(8) 1_565 . ?
O8 Cs3 O13W 141.3(9) . . ?
O18 Cs3 O13W 130.5(8) . . ?
O7 Cs3 O13W 97.7(8) . . ?
O7W Cs3 O13W 65.6(9) 1_565 . ?
O1W Cs3 Nb1 68.0(5) 2_566 . ?
O4W Cs3 Nb1 105.1(6) 1_565 . ?
O3W Cs3 Nb1 141.1(6) 1_565 . ?
O8 Cs3 Nb1 28.6(3) . . ?
O18 Cs3 Nb1 57.9(4) . . ?
O7 Cs3 Nb1 29.4(3) . . ?
O7W Cs3 Nb1 153.8(7) 1_565 . ?
O13W Cs3 Nb1 113.8(8) . . ?
O1W Cs3 Nb4 105.3(6) 2_566 . ?
O4W Cs3 Nb4 68.3(5) 1_565 . ?
O3W Cs3 Nb4 141.2(6) 1_565 . ?
O8 Cs3 Nb4 29.8(3) . . ?
O18 Cs3 Nb4 29.2(3) . . ?
O7 Cs3 Nb4 59.4(4) . . ?
O7W Cs3 Nb4 119.9(7) 1_565 . ?
O13W Cs3 Nb4 156.1(8) . . ?
Nb1 Cs3 Nb4 49.9(2) . . ?
O1W Cs3 K2 112.5(6) 2_566 1_565 ?
O4W Cs3 K2 43.3(4) 1_565 1_565 ?
O3W Cs3 K2 47.6(5) 1_565 1_565 ?
O8 Cs3 K2 119.5(6) . 1_565 ?
O18 Cs3 K2 108.6(5) . 1_565 ?
O7 Cs3 K2 157.7(6) . 1_565 ?
O7W Cs3 K2 48.1(7) 1_565 1_565 ?
O13W Cs3 K2 96.9(7) . 1_565 ?
Nb1 Cs3 K2 148.1(5) . 1_565 ?
Nb4 Cs3 K2 103.1(4) . 1_565 ?
O1W Cs3 K1 40.4(4) 2_566 2_566 ?
O4W Cs3 K1 113.5(6) 1_565 2_566 ?
O3W Cs3 K1 50.7(5) 1_565 2_566 ?
O8 Cs3 K1 115.4(5) . 2_566 ?
O18 Cs3 K1 153.1(6) . 2_566 ?
O7 Cs3 K1 103.8(5) . 2_566 ?
O7W Cs3 K1 94.8(6) 1_565 2_566 ?
O13W Cs3 K1 40.5(6) . 2_566 ?
Nb1 Cs3 K1 99.6(4) . 2_566 ?
Nb4 Cs3 K1 145.2(5) . 2_566 ?
K2 Cs3 K1 98.3(3) 1_565 2_566 ?
O1W K1 O13W 98.3(9) . 2_566 ?
O1W K1 O13 77.4(4) . . ?
O13W K1 O13 155.9(9) 2_566 . ?
O1W K1 O1P 152.0(6) . 2_556 ?
O13W K1 O1P 76.2(9) 2_566 2_556 ?
O13 K1 O1P 96.3(4) . 2_556 ?
O1W K1 O11W 148.2(9) . . ?
O13W K1 O11W 108.2(11) 2_566 . ?
O13 K1 O11W 84.8(7) . . ?
O1P K1 O11W 55.3(8) 2_556 . ?
O1W K1 O15W 127.0(11) . 2_456 ?
O13W K1 O15W 60.7(13) 2_566 2_456 ?
O13 K1 O15W 140.2(11) . 2_456 ?
O1P K1 O15W 74.8(11) 2_556 2_456 ?
O11W K1 O15W 57.9(12) . 2_456 ?
O1W K1 O2W 73.8(7) . . ?
O13W K1 O2W 121.4(10) 2_566 . ?
O13 K1 O2W 80.7(5) . . ?
O1P K1 O2W 132.8(7) 2_556 . ?
O11W K1 O2W 77.6(10) . . ?
O15W K1 O2W 78.2(12) 2_456 . ?
O1W K1 O3W 67.4(5) . 2_556 ?
O13W K1 O3W 71.4(9) 2_566 2_556 ?
O13 K1 O3W 85.3(4) . 2_556 ?
O1P K1 O3W 85.0(4) 2_556 2_556 ?
O11W K1 O3W 137.5(8) . 2_556 ?
O15W K1 O3W 130.9(11) 2_456 2_556 ?
O2W K1 O3W 140.7(6) . 2_556 ?
O1W K1 Nb6 88.5(4) . . ?
O13W K1 Nb6 131.2(9) 2_566 . ?
O13 K1 Nb6 26.5(3) . . ?
O1P K1 Nb6 75.8(3) 2_556 . ?
O11W K1 Nb6 87.0(7) . . ?
O15W K1 Nb6 143.1(10) 2_456 . ?
O2W K1 Nb6 107.0(5) . . ?
O3W K1 Nb6 67.1(3) 2_556 . ?
O1W K1 K4 113.7(4) . . ?
O13W K1 K4 147.9(8) 2_566 . ?
O13 K1 K4 44.1(3) . . ?
O1P K1 K4 76.0(3) 2_556 . ?
O11W K1 K4 41.3(7) . . ?
O15W K1 K4 96.6(10) 2_456 . ?
O2W K1 K4 69.5(6) . . ?
O3W K1 K4 121.4(3) 2_556 . ?
Nb6 K1 K4 54.60(16) . . ?
O1W K1 Cs3 40.0(5) . 2_566 ?
O13W K1 Cs3 61.7(8) 2_566 2_566 ?
O13 K1 Cs3 105.0(4) . 2_566 ?
O1P K1 Cs3 119.7(4) 2_556 2_566 ?
O11W K1 Cs3 169.8(7) . 2_566 ?
O15W K1 Cs3 113.1(10) 2_456 2_566 ?
O2W K1 Cs3 106.3(7) . 2_566 ?
O3W K1 Cs3 43.1(4) 2_556 2_566 ?
Nb6 K1 Cs3 100.6(3) . 2_566 ?
K4 K1 Cs3 148.8(3) . 2_566 ?
O1W K1 Cs2 47.5(4) . 2_566 ?
O13W K1 Cs2 53.0(8) 2_566 2_566 ?
O13 K1 Cs2 113.6(3) . 2_566 ?
O1P K1 Cs2 115.1(3) 2_556 2_566 ?
O11W K1 Cs2 161.0(7) . 2_566 ?
O15W K1 Cs2 105.0(10) 2_456 2_566 ?
O2W K1 Cs2 108.9(6) . 2_566 ?
O3W K1 Cs2 45.5(3) 2_556 2_566 ?
Nb6 K1 Cs2 107.34(15) . 2_566 ?
K4 K1 Cs2 157.6(2) . 2_566 ?
O12W K2 O4W 94.3(18) . . ?
O12W K2 O11W 96(2) . 2_456 ?
O4W K2 O11W 140.3(8) . 2_456 ?
O12W K2 O12 102.0(17) . . ?
O4W K2 O12 154.7(5) . . ?
O11W K2 O12 57.3(8) 2_456 . ?
O12W K2 O2P 157.8(17) . 2_556 ?
O4W K2 O2P 75.1(5) . 2_556 ?
O11W K2 O2P 81.0(8) 2_456 2_556 ?
O12 K2 O2P 95.1(4) . 2_556 ?
O12W K2 O2W 80.2(17) . 2_456 ?
O4W K2 O2W 63.6(8) . 2_456 ?
O11W K2 O2W 80.7(10) 2_456 2_456 ?
O12 K2 O2W 138.0(8) . 2_456 ?
O2P K2 O2W 77.6(6) 2_556 2_456 ?
O12W K2 O3W 113.5(19) . . ?
O4W K2 O3W 71.4(5) . . ?
O11W K2 O3W 136.0(8) 2_456 . ?
O12 K2 O3W 84.3(4) . . ?
O2P K2 O3W 82.0(4) 2_556 . ?
O2W K2 O3W 133.9(7) 2_456 . ?
O12W K2 O7W 49.0(18) . . ?
O4W K2 O7W 100.0(8) . . ?
O11W K2 O7W 115.7(10) 2_456 . ?
O12 K2 O7W 77.2(7) . . ?
O2P K2 O7W 151.0(7) 2_556 . ?
O2W K2 O7W 126.5(8) 2_456 . ?
O3W K2 O7W 69.5(7) . . ?
O12W K2 O15W 39(2) . . ?
O4W K2 O15W 124.1(10) . . ?
O11W K2 O15W 56.7(12) 2_456 . ?
O12 K2 O15W 79.7(10) . . ?
O2P K2 O15W 133.0(11) 2_556 . ?
O2W K2 O15W 76.3(11) 2_456 . ?
O3W K2 O15W 142.3(10) . . ?
O7W K2 O15W 73.7(12) . . ?
O12W K2 Nb6 125.5(17) . . ?
O4W K2 Nb6 130.4(4) . . ?
O11W K2 Nb6 70.1(7) 2_456 . ?
O12 K2 Nb6 26.0(3) . . ?
O2P K2 Nb6 74.5(3) 2_556 . ?
O2W K2 Nb6 142.1(6) 2_456 . ?
O3W K2 Nb6 66.3(3) . . ?
O7W K2 Nb6 88.7(6) . . ?
O15W K2 Nb6 105.3(9) . . ?
O12W K2 Cs3 80.1(19) . 1_545 ?
O4W K2 Cs3 43.5(5) . 1_545 ?
O11W K2 Cs3 175.3(8) 2_456 1_545 ?
O12 K2 Cs3 120.5(4) . 1_545 ?
O2P K2 Cs3 103.5(4) 2_556 1_545 ?
O2W K2 Cs3 101.3(7) 2_456 1_545 ?
O3W K2 Cs3 44.8(4) . 1_545 ?
O7W K2 Cs3 59.7(8) . 1_545 ?
O15W K2 Cs3 119.5(10) . 1_545 ?
Nb6 K2 Cs3 109.7(3) . 1_545 ?
O12W K2 K4 130.3(19) . 2_456 ?
O4W K2 K4 106.3(4) . 2_456 ?
O11W K2 K4 41.3(7) 2_456 2_456 ?
O12 K2 K4 77.6(3) . 2_456 ?
O2P K2 K4 40.4(4) 2_556 2_456 ?
O2W K2 K4 70.2(6) 2_456 2_456 ?
O3W K2 K4 115.8(3) . 2_456 ?
O7W K2 K4 153.5(7) . 2_456 ?
O15W K2 K4 93.8(10) . 2_456 ?
Nb6 K2 K4 71.91(16) . 2_456 ?
Cs3 K2 K4 143.4(3) 1_545 2_456 ?
O8W K3 O5W 85.5(7) . . ?
O8W K3 O10W 156.6(8) . . ?
O5W K3 O10W 91.5(8) . . ?
O8W K3 O9W 90.8(6) . . ?
O5W K3 O9W 155.1(6) . . ?
O10W K3 O9W 82.2(9) . . ?
O8W K3 O6W 75.0(6) . . ?
O5W K3 O6W 75.7(6) . . ?
O10W K3 O6W 81.8(8) . . ?
O9W K3 O6W 79.6(6) . . ?
O8W K3 O7W 75.9(7) . . ?
O5W K3 O7W 67.1(8) . . ?
O10W K3 O7W 124.1(9) . . ?
O9W K3 O7W 135.6(9) . . ?
O6W K3 O7W 133.9(8) . . ?
O8W K3 K5 112.0(4) . 2 ?
O5W K3 K5 114.9(4) . 2 ?
O10W K3 K5 49.0(7) . 2 ?
O9W K3 K5 44.6(5) . 2 ?
O6W K3 K5 53.0(5) . 2 ?
O7W K3 K5 171.8(6) . 2 ?
O8W K3 Cs1 46.3(5) . . ?
O5W K3 Cs1 45.9(5) . . ?
O10W K3 Cs1 118.3(7) . . ?
O9W K3 Cs1 117.2(4) . . ?
O6W K3 Cs1 50.6(5) . . ?
O7W K3 Cs1 83.5(6) . . ?
K5 K3 Cs1 103.6(2) 2 . ?
O8W K3 Cs2 82.0(5) . 1_545 ?
O5W K3 Cs2 104.0(4) . 1_545 ?
O10W K3 Cs2 121.1(7) . 1_545 ?
O9W K3 Cs2 99.8(5) . 1_545 ?
O6W K3 Cs2 156.9(5) . 1_545 ?
O7W K3 Cs2 37.1(7) . 1_545 ?
K5 K3 Cs2 139.2(2) 2 1_545 ?
Cs1 K3 Cs2 112.48(15) . 1_545 ?
O9W K5 O1 83.7(6) 2 . ?
O9W K5 O4 153.6(7) 2 1_655 ?
O1 K5 O4 110.9(5) . 1_655 ?
O9W K5 O2W 115.2(9) 2 2_566 ?
O1 K5 O2W 90.9(6) . 2_566 ?
O4 K5 O2W 87.3(7) 1_655 2_566 ?
O9W K5 O10W 79.1(8) 2 2 ?
O1 K5 O10W 156.9(8) . 2 ?
O4 K5 O10W 80.2(7) 1_655 2 ?
O2W K5 O10W 110.3(8) 2_566 2 ?
O9W K5 O6W 75.2(6) 2 2 ?
O1 K5 O6W 87.0(5) . 2 ?
O4 K5 O6W 83.5(5) 1_655 2 ?
O2W K5 O6W 169.1(8) 2_566 2 ?
O10W K5 O6W 73.9(7) 2 2 ?
O9W K5 K3 45.3(6) 2 2 ?
O1 K5 K3 112.7(4) . 2 ?
O4 K5 K3 108.4(4) 1_655 2 ?
O2W K5 K3 143.1(7) 2_566 2 ?
O10W K5 K3 44.4(6) 2 2 ?
O6W K5 K3 46.6(3) 2 2 ?
O9W K5 Nb1 67.6(4) 2 . ?
O1 K5 Nb1 20.4(3) . . ?
O4 K5 Nb1 120.0(4) 1_655 . ?
O2W K5 Nb1 108.8(6) 2_566 . ?
O10W K5 Nb1 136.5(7) 2 . ?
O6W K5 Nb1 71.2(4) 2 . ?
K3 K5 Nb1 92.24(19) 2 . ?
O9W K5 Nb4 133.7(6) 2 1_655 ?
O1 K5 Nb4 119.3(4) . 1_655 ?
O4 K5 Nb4 20.0(3) 1_655 1_655 ?
O2W K5 Nb4 104.8(6) 2_566 1_655 ?
O10W K5 Nb4 65.4(7) 2 1_655 ?
O6W K5 Nb4 67.3(4) 2 1_655 ?
K3 K5 Nb4 88.5(2) 2 1_655 ?
Nb1 K5 Nb4 120.9(2) . 1_655 ?
O9W K5 K1 76.6(6) 2 2_566 ?
O1 K5 K1 80.0(4) . 2_566 ?
O4 K5 K1 126.3(4) 1_655 2_566 ?
O2W K5 K1 39.2(6) 2_566 2_566 ?
O10W K5 K1 110.4(7) 2 2_566 ?
O6W K5 K1 150.0(4) 2 2_566 ?
K3 K5 K1 115.0(2) 2 2_566 ?
Nb1 K5 K1 88.73(17) . 2_566 ?
Nb4 K5 K1 142.3(2) 1_655 2_566 ?
O9W K5 K2 108.1(5) 2 1_665 ?
O1 K5 K2 126.9(4) . 1_665 ?
O4 K5 K2 81.2(3) 1_655 1_665 ?
O2W K5 K2 36.7(5) 2_566 1_665 ?
O10W K5 K2 73.6(6) 2 1_665 ?
O6W K5 K2 146.0(4) 2 1_665 ?
K3 K5 K2 111.2(2) 2 1_665 ?
Nb1 K5 K2 142.3(2) . 1_665 ?
Nb4 K5 K2 89.93(16) 1_655 1_665 ?
K1 K5 K2 55.02(14) 2_566 1_665 ?
O11W K4 O2P 127.4(13) 2_456 1_455 ?
O11W K4 O1P 68.3(13) 2_456 1_455 ?
O2P K4 O1P 62.7(5) 1_455 1_455 ?
O11W K4 O11W 104.8(12) 2_456 . ?
O2P K4 O11W 84.4(9) 1_455 . ?
O1P K4 O11W 119.8(9) 1_455 . ?
O11W K4 O19 103.6(12) 2_456 . ?
O2P K4 O19 98.6(5) 1_455 . ?
O1P K4 O19 94.8(5) 1_455 . ?
O11W K4 O19 141.4(9) . . ?
O11W K4 O13 116.0(13) 2_456 . ?
O2P K4 O13 116.2(6) 1_455 . ?
O1P K4 O13 152.2(5) 1_455 . ?
O11W K4 O13 86.6(9) . . ?
O19 K4 O13 57.4(4) . . ?
O11W K4 K4 66.5(11) 2_456 2_456 ?
O2P K4 K4 107.2(6) 1_455 2_456 ?
O1P K4 K4 103.6(5) 1_455 2_456 ?
O11W K4 K4 38.3(8) . 2_456 ?
O19 K4 K4 153.1(6) . 2_456 ?
O13 K4 K4 103.0(5) . 2_456 ?
O11W K4 O12 61.8(12) 2_456 . ?
O2P K4 O12 154.1(5) 1_455 . ?
O1P K4 O12 109.7(6) 1_455 . ?
O11W K4 O12 118.5(9) . . ?
O19 K4 O12 56.2(4) . . ?
O13 K4 O12 57.9(4) . . ?
K4 K4 O12 98.6(5) 2_456 . ?
O11W K4 Pt1 96.5(13) 2_456 1_455 ?
O2P K4 Pt1 31.5(3) 1_455 1_455 ?
O1P K4 Pt1 32.2(4) 1_455 1_455 ?
O11W K4 Pt1 98.7(9) . 1_455 ?
O19 K4 Pt1 103.5(4) . 1_455 ?
O13 K4 Pt1 144.6(4) . 1_455 ?
K4 K4 Pt1 102.5(4) 2_456 1_455 ?
O12 K4 Pt1 140.0(4) . 1_455 ?
O11W K4 Nb6 85.4(13) 2_456 . ?
O2P K4 Nb6 146.4(5) 1_455 . ?
O1P K4 Nb6 140.3(5) 1_455 . ?
O11W K4 Nb6 94.7(9) . . ?
O19 K4 Nb6 62.1(3) . . ?
O13 K4 Nb6 30.6(3) . . ?
K4 K4 Nb6 91.5(4) 2_456 . ?
O12 K4 Nb6 30.9(3) . . ?
Pt1 K4 Nb6 165.4(3) 1_455 . ?
O11W K4 Nb4 125.5(12) 2_456 . ?
O2P K4 Nb4 96.6(4) 1_455 . ?
O1P K4 Nb4 121.3(4) 1_455 . ?
O11W K4 Nb4 110.7(8) . . ?
O19 K4 Nb4 30.7(3) . . ?
O13 K4 Nb4 32.3(3) . . ?
K4 K4 Nb4 135.1(5) 2_456 . ?
O12 K4 Nb4 65.2(3) . . ?
Pt1 K4 Nb4 116.7(3) 1_455 . ?
Nb6 K4 Nb4 52.36(12) . . ?
O11W K4 Nb5 75.8(12) 2_456 . ?
O2P K4 Nb5 122.9(4) 1_455 . ?
O1P K4 Nb5 92.3(4) 1_455 . ?
O11W K4 Nb5 146.2(9) . . ?
O19 K4 Nb5 29.0(3) . . ?
O13 K4 Nb5 64.3(3) . . ?
K4 K4 Nb5 129.1(5) 2_456 . ?
O12 K4 Nb5 31.4(3) . . ?
Pt1 K4 Nb5 114.9(3) 1_455 . ?
Nb6 K4 Nb5 51.45(12) . . ?
Nb4 K4 Nb5 51.78(12) . . ?
Pt1 O16 Nb1 100.0(5) . . ?
Pt1 O16 Nb6 99.9(6) . . ?
Nb1 O16 Nb6 109.7(6) . . ?
Nb6 O15 Pt1 178.5(8) . 2_556 ?
Pt1 O14 Nb6 100.2(6) . . ?
Pt1 O14 Nb2 98.9(6) . . ?
Nb6 O14 Nb2 110.7(6) . . ?
Nb6 O13 Nb4 113.2(6) . . ?
Nb6 O13 K1 112.9(5) . . ?
Nb4 O13 K1 129.4(6) . . ?
Nb6 O13 K4 99.5(5) . . ?
Nb4 O13 K4 98.5(5) . . ?
K1 O13 K4 93.4(4) . . ?
Nb6 O12 Nb5 112.7(6) . . ?
Nb6 O12 K2 114.2(6) . . ?
Nb5 O12 K2 128.7(6) . . ?
Nb6 O12 K4 95.8(5) . . ?
Nb5 O12 K4 98.9(5) . . ?
K2 O12 K4 96.0(4) . . ?
Pt1 O2P K4 103.9(7) . 1_655 ?
Pt1 O2P K2 122.0(7) . 2_556 ?
K4 O2P K2 96.8(5) 1_655 2_556 ?
Pt1 O1P K4 102.0(6) . 1_655 ?
Pt1 O1P K1 118.7(6) . 2_556 ?
K4 O1P K1 99.5(5) 1_655 2_556 ?
Nb5 O11 Cs1 128.0(8) . 2_455 ?
Nb6 O10 Nb4 90.1(4) . . ?
Nb6 O10 Nb1 95.5(5) . . ?
Nb4 O10 Nb1 88.8(4) . . ?
Nb6 O10 Nb5 89.5(4) . . ?
Nb4 O10 Nb5 88.4(4) . . ?
Nb1 O10 Nb5 174.3(6) . . ?
Nb6 O10 Nb2 95.0(5) . . ?
Nb4 O10 Nb2 173.4(6) . . ?
Nb1 O10 Nb2 94.8(5) . . ?
Nb5 O10 Nb2 87.5(4) . . ?
Nb6 O10 Nb7 176.6(6) . . ?
Nb4 O10 Nb7 87.8(4) . . ?
Nb1 O10 Nb7 87.1(4) . . ?
Nb5 O10 Nb7 87.8(4) . . ?
Nb2 O10 Nb7 86.9(4) . . ?
Pt1 O9 Nb1 98.8(5) . . ?
Pt1 O9 Nb2 98.4(6) . . ?
Nb1 O9 Nb2 112.5(6) . . ?
Nb1 O8 Nb4 114.5(7) . . ?
Nb1 O8 Cs3 103.2(6) . . ?
Nb4 O8 Cs3 103.7(6) . . ?
Nb1 O8 Cs2 97.6(5) . . ?
Nb4 O8 Cs2 100.1(5) . . ?
Nb1 O7 Nb7 116.2(7) . . ?
Nb1 O7 Cs2 104.0(7) . . ?
Nb7 O7 Cs2 99.4(6) . . ?
Nb1 O7 Cs3 92.8(7) . . ?
Nb7 O7 Cs3 103.8(7) . . ?
Nb2 O6 Nb7 117.1(7) . . ?
Nb2 O6 Cs1 102.1(6) . . ?
Nb7 O6 Cs1 99.9(5) . . ?
Nb2 O5 Cs1 127.2(7) . 2 ?
Nb4 O4 K5 127.1(7) . 1_455 ?
Nb2 O3 Nb5 116.5(7) . . ?
Nb2 O3 Cs1 96.8(5) . . ?
Nb5 O3 Cs1 99.9(5) . . ?
Nb1 O1 K5 126.4(7) . . ?
Nb7 O18 Nb4 117.1(8) . . ?
Nb7 O18 Cs2 102.8(6) . . ?
Nb4 O18 Cs2 110.5(6) . . ?
Nb7 O18 Cs3 109.6(6) . . ?
Nb4 O18 Cs3 98.8(7) . . ?
Nb4 O19 Nb5 117.1(7) . . ?
Nb4 O19 K4 100.9(5) . . ?
Nb5 O19 K4 105.7(6) . . ?
Nb5 O17 Nb7 117.2(7) . . ?
Nb5 O17 Cs1 108.4(7) . . ?
Nb7 O17 Cs1 101.4(6) . . ?
Cs3 O3W K2 87.6(6) 1_545 . ?
K2 O3W Cs2 88.4(5) . 1_545 ?
Cs3 O3W K1 86.2(6) 1_545 2_556 ?
K2 O3W K1 173.5(6) . 2_556 ?
Cs2 O3W K1 85.1(5) 1_545 2_556 ?
K3 O5W Cs1 92.2(6) . . ?
K3 O6W Cs1 83.5(5) . . ?
K3 O6W K5 80.4(5) . 2 ?
Cs1 O6W K5 163.8(6) . 2 ?
Cs3 O1W K1 99.6(7) 2_566 . ?
K1 O1W Cs2 92.3(5) . 2_566 ?
K3 O8W Cs1 91.9(6) . . ?
K2 O4W Cs3 93.3(6) . 1_545 ?
K2 O4W Cs2 87.4(5) . 1_545 ?
K5 O9W K3 90.1(8) 2 . ?
K5 O2W K2 107.9(8) 2_566 2_456 ?
K5 O2W K1 104.0(8) 2_566 . ?
K2 O2W K1 92.5(10) 2_456 . ?
K3 O10W K5 86.6(9) . 2 ?
K4 O11W K4 75.2(12) 2_456 . ?
K4 O11W K2 135.9(18) 2_456 2_456 ?
K4 O11W K2 96.6(12) . 2_456 ?
K4 O11W K1 124.2(18) 2_456 . ?
K4 O11W K1 94.0(11) . . ?
K2 O11W K1 99.3(11) 2_456 . ?
K2 O7W K3 160.5(13) . . ?
K2 O7W Cs2 81.0(8) . 1_545 ?
K3 O7W Cs2 106.0(11) . 1_545 ?
K2 O7W Cs3 72.2(7) . 1_545 ?
K3 O7W Cs3 114.6(11) . 1_545 ?
K1 O13W Cs2 86.4(10) 2_566 . ?
K1 O13W Cs3 77.9(9) 2_566 . ?
K1 O15W K2 89.9(13) 2_456 . ?

_refine_diff_density_max         4.298
_refine_diff_density_min         -2.968
_refine_diff_density_rms         0.424

_shelxl_version_number           2013-4


_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_standards_number         0
_diffrn_standards_decay_%        0

 
data_3
#complex Na2K10-2
_audit_creation_method           SHELXL-2013
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'H36 K10 Na2 Nb12 O56 Pt'
_chemical_formula_weight         2679.28

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -2.0727 0.6215 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pt Pt -1.7033 8.3905 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      cubic
_space_group_IT_number           205
_symmetry_space_group_name_H-M   'P a -3'
_space_group_name_Hall           '-P 2ac 2ab 3'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'z, x, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z, x'
'-y, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z, x+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z-1/2'
'-x-1/2, y-1/2, z'
'-z, -x, -y'
'-z-1/2, x-1/2, y'
'z-1/2, x, -y-1/2'
'z, -x-1/2, y-1/2'
'-y, -z, -x'
'y, -z-1/2, x-1/2'
'-y-1/2, z-1/2, x'
'y-1/2, z, -x-1/2'

_cell_length_a                   18.1811(6)
_cell_length_b                   18.1811(6)
_cell_length_c                   18.1811(6)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     6009.8(6)
_cell_formula_units_Z            4
_cell_measurement_temperature    150(2)
_cell_measurement_reflns_used    9942
_cell_measurement_theta_min      2.24
_cell_measurement_theta_max      26.99

_exptl_crystal_description       polyhedra
_exptl_crystal_colour            light-yellow
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    2.961
_exptl_crystal_F_000             5064
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.100
_exptl_crystal_size_mid          0.080
_exptl_crystal_size_min          0.080
_exptl_absorpt_coefficient_mu    5.334
_shelx_estimated_absorpt_T_min   0.618
_shelx_estimated_absorpt_T_max   0.675
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.618
_exptl_absorpt_correction_T_max  0.675
_exptl_absorpt_process_details   'SADABS (Bruker-AXS, 2004)'

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      150(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Nonius X8Apex CCD'
_diffrn_measurement_method       'φ scans'
_diffrn_detector_area_resol_mean 25
_diffrn_reflns_number            81602
_diffrn_reflns_av_unetI/netI     0.0151
_diffrn_reflns_av_R_equivalents  0.0566
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_theta_min         1.940
_diffrn_reflns_theta_max         27.498
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measured_fraction_theta_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_point_group_measured_fraction_full 1.000
_reflns_number_total             2311
_reflns_number_gt                2004
_reflns_threshold_expression     >2σ(I)
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_computing_data_collection       'APEX2 (Bruker-AXS, 2004)'
_computing_cell_refinement       'SAINT (Bruker-AXS, 2004)'
_computing_data_reduction        'SAINT (Bruker-AXS, 2004)'
_computing_structure_solution    'SHELXS-2013'
_computing_structure_refinement  'SHELXL-2013'
_computing_molecular_graphics    'SHELXTL (Bruker-AXS, 2004)'
_computing_publication_material  'CIFTAB-97 (Sheldrick, 1998)'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0860P)²+62.0731P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         2311
_refine_ls_number_parameters     144
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0480
_refine_ls_R_factor_gt           0.0394
_refine_ls_wR_factor_ref         0.1429
_refine_ls_wR_factor_gt          0.1322
_refine_ls_goodness_of_fit_ref   1.073
_refine_ls_restrained_S_all      1.073
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Pt1 Pt 0.5000 0.0000 0.0000 0.0190(2) Uani 1 6 d S T P . .
Nb1 Nb 0.43511(4) 0.16248(4) -0.00746(3) 0.0222(2) Uani 1 1 d . . . . .
Nb2 Nb 0.26852(4) 0.17563(4) -0.08273(4) 0.0256(2) Uani 1 1 d . . . . .
O7 O 0.5191(3) 0.0967(3) -0.0533(3) 0.0220(10) Uani 1 1 d . . . . .
O6 O 0.1841(3) 0.2158(4) -0.0571(4) 0.0429(15) Uani 1 1 d . . . . .
O5 O 0.3352(3) 0.1922(3) 0.0050(3) 0.0277(11) Uani 1 1 d . . . . .
O4 O 0.4599(3) 0.2414(3) -0.0728(3) 0.0276(11) Uani 1 1 d . . . . .
O3 O 0.3812(3) 0.1188(3) -0.1188(3) 0.0225(17) Uani 1 3 d S T P . .
O2 O 0.4744(3) 0.1894(3) 0.0777(3) 0.0337(12) Uani 1 1 d . . . . .
O1 O 0.2436(3) 0.1312(3) -0.1795(3) 0.0301(12) Uani 1 1 d . . . . .
K1 K 0.61124(12) 0.17052(12) 0.12716(14) 0.0465(5) Uani 1 1 d . . . . .
Na1 Na 0.67402(18) 0.17402(18) 0.32598(18) 0.0270(11) Uani 1 3 d S T P . .
O1W O 0.6286(4) 0.2835(4) 0.2373(5) 0.058(2) Uani 1 1 d . . . . .
O2W O 0.6089(5) 0.2396(7) 0.4333(5) 0.088(3) Uani 1 1 d . . . . .
K2A K 0.4995(4) 0.3459(4) 0.1299(4) 0.0376(15) Uani 0.4 1 d . . P . 1
K2B K 0.4694(6) 0.3544(6) 0.1190(5) 0.039(2) Uani 0.2665 1 d . . P . 2
O3W O 0.5853(18) 0.4106(17) 0.038(2) 0.112(12) Uani 0.55 1 d . . P . .
O6W O 0.5000 0.5000 0.0000 0.02(5) Uiso 0.06 6 d S . P . .
O5W O 0.584(4) 0.401(3) 0.067(3) 0.080(14) Uiso 0.32 1 d . . P . .
O4W O 0.576(4) 0.334(4) -0.043(4) 0.069(19) Uiso 0.12 1 d . . P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Pt1 O7 2.038(5) 18_655 ?
Pt1 O7 2.038(5) 6 ?
Pt1 O7 2.038(5) 13_655 ?
Pt1 O7 2.038(5) 24_656 ?
Pt1 O7 2.038(5) 12_554 ?
Pt1 O7 2.038(5) . ?
Pt1 Nb1 3.1838(7) 12_554 ?
Pt1 Nb1 3.1838(7) 24_656 ?
Pt1 Nb1 3.1838(7) 6 ?
Pt1 Nb1 3.1838(7) 18_655 ?
Pt1 Nb1 3.1838(7) 13_655 ?
Pt1 Nb1 3.1838(7) . ?
Nb1 O2 1.774(5) . ?
Nb1 O5 1.908(5) . ?
Nb1 O4 1.917(5) . ?
Nb1 O7 2.111(5) . ?
Nb1 O7 2.123(5) 12_554 ?
Nb1 O3 2.385(4) . ?
Nb1 Nb2 3.3207(9) 6 ?
Nb1 Nb2 3.3321(9) . ?
Nb1 K1 3.553(2) 18_655 ?
Nb1 K1 4.033(2) . ?
Nb1 K2A 4.110(7) 22_565 ?
Nb2 O6 1.763(6) . ?
Nb2 O1 1.957(6) 6 ?
Nb2 O1 1.988(6) . ?
Nb2 O5 2.026(5) . ?
Nb2 O4 2.031(5) 12_554 ?
Nb2 O3 2.386(5) . ?
Nb2 Nb1 3.3208(9) 12_554 ?
Nb2 Nb2 3.3463(12) 6 ?
Nb2 Nb2 3.3463(12) 12_554 ?
Nb2 K2B 3.956(9) 20_565 ?
Nb2 K1 4.081(2) 4_455 ?
O7 Nb1 2.123(5) 6 ?
O7 K1 2.999(5) 24_656 ?
O6 K1 2.766(7) 4_455 ?
O5 K2A 3.242(9) 22_565 ?
O5 K1 3.419(6) 18_655 ?
O4 Nb2 2.031(5) 6 ?
O4 K2B 3.271(11) 22_565 ?
O4 K2A 3.390(9) 22_565 ?
O3 Nb1 2.385(4) 12_554 ?
O3 Nb1 2.385(4) 6 ?
O3 Nb2 2.386(5) 12_554 ?
O3 Nb2 2.386(5) 6 ?
O2 K1 2.668(6) . ?
O2 K1 2.876(7) 18_655 ?
O2 K2A 3.035(9) . ?
O2 K2B 3.094(12) . ?
O1 Nb2 1.957(6) 12_554 ?
O1 K2B 2.975(11) 20_565 ?
O1 K2A 3.184(10) 20_565 ?
K1 O6 2.766(7) 4 ?
K1 O2W 2.788(14) 8_645 ?
K1 O2 2.876(7) 24_656 ?
K1 O1W 2.885(8) . ?
K1 O7 2.999(5) 18_655 ?
K1 O1W 3.288(9) 8_645 ?
K1 O5 3.419(6) 24_656 ?
K1 Nb1 3.553(2) 24_656 ?
K1 K2A 3.781(7) . ?
K1 Na1 3.791(3) . ?
Na1 O2W 2.574(10) 8_645 ?
Na1 O2W 2.574(10) 11_556 ?
Na1 O2W 2.575(10) . ?
Na1 O1W 2.691(9) 11_556 ?
Na1 O1W 2.691(9) 8_645 ?
Na1 O1W 2.691(9) . ?
Na1 O4W 2.98(8) 18_655 ?
Na1 O4W 2.98(8) 21_656 ?
Na1 O4W 2.98(8) 15_566 ?
Na1 K1 3.791(3) 11_556 ?
Na1 K1 3.791(3) 8_645 ?
O1W K2A 3.257(11) . ?
O1W K1 3.288(9) 11_556 ?
O2W O4W 1.53(8) 15_566 ?
O2W K1 2.788(14) 11_556 ?
K2A O5W 2.17(6) . ?
K2A O5W 2.52(7) 22_565 ?
K2A O3W 2.57(4) . ?
K2A O3W 2.78(4) 22_565 ?
K2A O1 3.184(10) 23_665 ?
K2A O5 3.242(9) 19_656 ?
K2A O4 3.390(9) 19_656 ?
K2A K2A 3.689(7) 19_656 ?
K2A K2A 3.689(7) 22_565 ?
K2B O5W 1.99(6) 22_565 ?
K2B O3W 2.32(4) 22_565 ?
K2B O5W 2.45(6) . ?
K2B O3W 2.77(4) . ?
K2B O1 2.975(11) 23_665 ?
K2B O4 3.271(11) 19_656 ?
K2B K2B 3.465(10) 22_565 ?
K2B K2B 3.465(10) 19_656 ?
K2B Nb2 3.956(9) 23_665 ?
K2B Nb2 4.156(9) 19_656 ?
O3W O5W 0.56(7) . ?
O3W K2B 2.32(4) 19_656 ?
O3W K2A 2.78(4) 19_656 ?
O5W K2B 1.99(6) 19_656 ?
O5W K2A 2.52(7) 19_656 ?
O4W O2W 1.53(8) 15_565 ?
O4W Na1 2.98(8) 15_565 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O7 Pt1 O7 180.0(3) 18_655 6 ?
O7 Pt1 O7 79.5(2) 18_655 13_655 ?
O7 Pt1 O7 100.5(2) 6 13_655 ?
O7 Pt1 O7 79.5(2) 18_655 24_656 ?
O7 Pt1 O7 100.5(2) 6 24_656 ?
O7 Pt1 O7 79.5(2) 13_655 24_656 ?
O7 Pt1 O7 100.5(2) 18_655 12_554 ?
O7 Pt1 O7 79.5(2) 6 12_554 ?
O7 Pt1 O7 100.5(2) 13_655 12_554 ?
O7 Pt1 O7 180.0(4) 24_656 12_554 ?
O7 Pt1 O7 100.5(2) 18_655 . ?
O7 Pt1 O7 79.5(2) 6 . ?
O7 Pt1 O7 180.0 13_655 . ?
O7 Pt1 O7 100.5(2) 24_656 . ?
O7 Pt1 O7 79.5(2) 12_554 . ?
O7 Pt1 Nb1 138.92(14) 18_655 12_554 ?
O7 Pt1 Nb1 41.08(14) 6 12_554 ?
O7 Pt1 Nb1 93.15(14) 13_655 12_554 ?
O7 Pt1 Nb1 139.27(14) 24_656 12_554 ?
O7 Pt1 Nb1 40.73(14) 12_554 12_554 ?
O7 Pt1 Nb1 86.85(14) . 12_554 ?
O7 Pt1 Nb1 41.08(14) 18_655 24_656 ?
O7 Pt1 Nb1 138.92(14) 6 24_656 ?
O7 Pt1 Nb1 86.85(14) 13_655 24_656 ?
O7 Pt1 Nb1 40.73(14) 24_656 24_656 ?
O7 Pt1 Nb1 139.27(14) 12_554 24_656 ?
O7 Pt1 Nb1 93.15(14) . 24_656 ?
Nb1 Pt1 Nb1 180.00(3) 12_554 24_656 ?
O7 Pt1 Nb1 139.27(14) 18_655 6 ?
O7 Pt1 Nb1 40.73(14) 6 6 ?
O7 Pt1 Nb1 138.92(14) 13_655 6 ?
O7 Pt1 Nb1 93.15(14) 24_656 6 ?
O7 Pt1 Nb1 86.85(14) 12_554 6 ?
O7 Pt1 Nb1 41.08(14) . 6 ?
Nb1 Pt1 Nb1 66.474(18) 12_554 6 ?
Nb1 Pt1 Nb1 113.526(18) 24_656 6 ?
O7 Pt1 Nb1 40.73(14) 18_655 18_655 ?
O7 Pt1 Nb1 139.27(14) 6 18_655 ?
O7 Pt1 Nb1 41.08(14) 13_655 18_655 ?
O7 Pt1 Nb1 86.85(14) 24_656 18_655 ?
O7 Pt1 Nb1 93.15(14) 12_554 18_655 ?
O7 Pt1 Nb1 138.92(14) . 18_655 ?
Nb1 Pt1 Nb1 113.526(18) 12_554 18_655 ?
Nb1 Pt1 Nb1 66.474(18) 24_656 18_655 ?
Nb1 Pt1 Nb1 180.00(3) 6 18_655 ?
O7 Pt1 Nb1 86.85(14) 18_655 13_655 ?
O7 Pt1 Nb1 93.15(14) 6 13_655 ?
O7 Pt1 Nb1 40.73(14) 13_655 13_655 ?
O7 Pt1 Nb1 41.08(14) 24_656 13_655 ?
O7 Pt1 Nb1 138.92(14) 12_554 13_655 ?
O7 Pt1 Nb1 139.27(14) . 13_655 ?
Nb1 Pt1 Nb1 113.526(18) 12_554 13_655 ?
Nb1 Pt1 Nb1 66.474(18) 24_656 13_655 ?
Nb1 Pt1 Nb1 113.526(18) 6 13_655 ?
Nb1 Pt1 Nb1 66.474(18) 18_655 13_655 ?
O7 Pt1 Nb1 93.15(14) 18_655 . ?
O7 Pt1 Nb1 86.85(14) 6 . ?
O7 Pt1 Nb1 139.27(14) 13_655 . ?
O7 Pt1 Nb1 138.92(14) 24_656 . ?
O7 Pt1 Nb1 41.08(14) 12_554 . ?
O7 Pt1 Nb1 40.73(14) . . ?
Nb1 Pt1 Nb1 66.476(18) 12_554 . ?
Nb1 Pt1 Nb1 113.524(18) 24_656 . ?
Nb1 Pt1 Nb1 66.475(18) 6 . ?
Nb1 Pt1 Nb1 113.525(18) 18_655 . ?
Nb1 Pt1 Nb1 180.0 13_655 . ?
O2 Nb1 O5 101.6(3) . . ?
O2 Nb1 O4 103.9(3) . . ?
O5 Nb1 O4 94.9(2) . . ?
O2 Nb1 O7 102.1(2) . . ?
O5 Nb1 O7 153.6(2) . . ?
O4 Nb1 O7 90.5(2) . . ?
O2 Nb1 O7 99.7(2) . 12_554 ?
O5 Nb1 O7 88.8(2) . 12_554 ?
O4 Nb1 O7 154.8(2) . 12_554 ?
O7 Nb1 O7 76.0(3) . 12_554 ?
O2 Nb1 O3 176.4(2) . . ?
O5 Nb1 O3 78.69(19) . . ?
O4 Nb1 O3 79.62(19) . . ?
O7 Nb1 O3 76.91(19) . . ?
O7 Nb1 O3 76.69(19) 12_554 . ?
O2 Nb1 Pt1 94.0(2) . . ?
O5 Nb1 Pt1 127.62(18) . . ?
O4 Nb1 Pt1 129.35(16) . . ?
O7 Nb1 Pt1 39.04(14) . . ?
O7 Nb1 Pt1 39.09(13) 12_554 . ?
O3 Nb1 Pt1 83.08(17) . . ?
O2 Nb1 Nb2 137.6(2) . 6 ?
O5 Nb1 Nb2 84.79(16) . 6 ?
O4 Nb1 Nb2 33.83(16) . 6 ?
O7 Nb1 Nb2 85.47(14) . 6 ?
O7 Nb1 Nb2 122.41(13) 12_554 6 ?
O3 Nb1 Nb2 45.91(12) . 6 ?
Pt1 Nb1 Nb2 115.21(2) . 6 ?
O2 Nb1 Nb2 134.8(2) . . ?
O5 Nb1 Nb2 33.21(16) . . ?
O4 Nb1 Nb2 84.55(16) . . ?
O7 Nb1 Nb2 122.41(14) . . ?
O7 Nb1 Nb2 85.00(13) 12_554 . ?
O3 Nb1 Nb2 45.72(12) . . ?
Pt1 Nb1 Nb2 114.89(2) . . ?
Nb2 Nb1 Nb2 60.40(3) 6 . ?
O2 Nb1 K1 53.5(2) . 18_655 ?
O5 Nb1 K1 70.31(17) . 18_655 ?
O4 Nb1 K1 146.70(17) . 18_655 ?
O7 Nb1 K1 116.21(14) . 18_655 ?
O7 Nb1 K1 57.37(14) 12_554 18_655 ?
O3 Nb1 K1 123.69(6) . 18_655 ?
Pt1 Nb1 K1 80.56(4) . 18_655 ?
Nb2 Nb1 K1 155.04(5) 6 18_655 ?
Nb2 Nb1 K1 95.93(4) . 18_655 ?
O2 Nb1 K1 30.8(2) . . ?
O5 Nb1 K1 132.33(16) . . ?
O4 Nb1 K1 99.36(16) . . ?
O7 Nb1 K1 71.69(14) . . ?
O7 Nb1 K1 96.45(13) 12_554 . ?
O3 Nb1 K1 148.58(13) . . ?
Pt1 Nb1 K1 73.35(3) . . ?
Nb2 Nb1 K1 128.51(4) 6 . ?
Nb2 Nb1 K1 165.54(4) . . ?
K1 Nb1 K1 73.13(2) 18_655 . ?
O2 Nb1 K2A 83.0(2) . 22_565 ?
O5 Nb1 K2A 50.3(2) . 22_565 ?
O4 Nb1 K2A 54.84(19) . 22_565 ?
O7 Nb1 K2A 144.86(17) . 22_565 ?
O7 Nb1 K2A 138.08(17) 12_554 22_565 ?
O3 Nb1 K2A 99.8(2) . 22_565 ?
Pt1 Nb1 K2A 175.54(10) . 22_565 ?
Nb2 Nb1 K2A 69.08(10) 6 22_565 ?
Nb2 Nb1 K2A 65.68(11) . 22_565 ?
K1 Nb1 K2A 94.99(10) 18_655 22_565 ?
K1 Nb1 K2A 105.14(11) . 22_565 ?
O6 Nb2 O1 103.3(3) . 6 ?
O6 Nb2 O1 101.7(3) . . ?
O1 Nb2 O1 90.9(3) 6 . ?
O6 Nb2 O5 104.6(3) . . ?
O1 Nb2 O5 87.4(2) 6 . ?
O1 Nb2 O5 153.3(2) . . ?
O6 Nb2 O4 101.7(3) . 12_554 ?
O1 Nb2 O4 154.9(2) 6 12_554 ?
O1 Nb2 O4 86.8(2) . 12_554 ?
O5 Nb2 O4 83.7(2) . 12_554 ?
O6 Nb2 O3 178.6(3) . . ?
O1 Nb2 O3 77.67(19) 6 . ?
O1 Nb2 O3 77.11(19) . . ?
O5 Nb2 O3 76.51(19) . . ?
O4 Nb2 O3 77.46(19) 12_554 . ?
O6 Nb2 Nb1 133.2(2) . 12_554 ?
O1 Nb2 Nb1 123.55(16) 6 12_554 ?
O1 Nb2 Nb1 78.39(16) . 12_554 ?
O5 Nb2 Nb1 80.44(16) . 12_554 ?
O4 Nb2 Nb1 31.71(15) 12_554 12_554 ?
O3 Nb2 Nb1 45.88(11) . 12_554 ?
O6 Nb2 Nb1 135.5(2) . . ?
O1 Nb2 Nb1 78.46(16) 6 . ?
O1 Nb2 Nb1 122.80(16) . . ?
O5 Nb2 Nb1 31.05(15) . . ?
O4 Nb2 Nb1 81.86(15) 12_554 . ?
O3 Nb2 Nb1 45.69(11) . . ?
Nb1 Nb2 Nb1 63.28(2) 12_554 . ?
O6 Nb2 Nb2 135.4(2) . 6 ?
O1 Nb2 Nb2 32.25(16) 6 6 ?
O1 Nb2 Nb2 82.01(17) . 6 ?
O5 Nb2 Nb2 82.44(16) . 6 ?
O4 Nb2 Nb2 122.94(15) 12_554 6 ?
O3 Nb2 Nb2 45.48(11) . 6 ?
Nb1 Nb2 Nb2 91.336(16) 12_554 6 ?
Nb1 Nb2 Nb2 59.634(19) . 6 ?
O6 Nb2 Nb2 133.4(2) . 12_554 ?
O1 Nb2 Nb2 82.42(17) 6 12_554 ?
O1 Nb2 Nb2 31.69(16) . 12_554 ?
O5 Nb2 Nb2 121.97(15) . 12_554 ?
O4 Nb2 Nb2 82.57(15) 12_554 12_554 ?
O3 Nb2 Nb2 45.48(11) . 12_554 ?
Nb1 Nb2 Nb2 59.97(2) 12_554 12_554 ?
Nb1 Nb2 Nb2 91.139(16) . 12_554 ?
Nb2 Nb2 Nb2 60.0 6 12_554 ?
O6 Nb2 K2B 75.8(3) . 20_565 ?
O1 Nb2 K2B 134.6(2) 6 20_565 ?
O1 Nb2 K2B 46.9(2) . 20_565 ?
O5 Nb2 K2B 137.6(2) . 20_565 ?
O4 Nb2 K2B 55.6(2) 12_554 20_565 ?
O3 Nb2 K2B 102.81(16) . 20_565 ?
Nb1 Nb2 K2B 70.97(18) 12_554 20_565 ?
Nb1 Nb2 K2B 134.05(18) . 20_565 ?
Nb2 Nb2 K2B 127.71(15) 6 20_565 ?
Nb2 Nb2 K2B 68.80(15) 12_554 20_565 ?
O6 Nb2 K1 32.7(2) . 4_455 ?
O1 Nb2 K1 74.62(16) 6 4_455 ?
O1 Nb2 K1 86.74(16) . 4_455 ?
O5 Nb2 K1 118.25(16) . 4_455 ?
O4 Nb2 K1 130.06(15) 12_554 4_455 ?
O3 Nb2 K1 147.56(16) . 4_455 ?
Nb1 Nb2 K1 156.22(4) 12_554 4_455 ?
Nb1 Nb2 K1 140.12(4) . 4_455 ?
Nb2 Nb2 K1 104.98(3) 6 4_455 ?
Nb2 Nb2 K1 113.49(4) 12_554 4_455 ?
K2B Nb2 K1 85.31(18) 20_565 4_455 ?
Pt1 O7 Nb1 100.2(2) . . ?
Pt1 O7 Nb1 99.8(2) . 6 ?
Nb1 O7 Nb1 111.0(2) . 6 ?
Pt1 O7 K1 118.9(2) . 24_656 ?
Nb1 O7 K1 134.3(2) . 24_656 ?
Nb1 O7 K1 86.03(17) 6 24_656 ?
Nb2 O6 K1 127.2(3) . 4_455 ?
Nb1 O5 Nb2 115.7(3) . . ?
Nb1 O5 K2A 102.8(3) . 22_565 ?
Nb2 O5 K2A 99.2(2) . 22_565 ?
Nb1 O5 K1 78.00(18) . 18_655 ?
Nb2 O5 K1 138.5(3) . 18_655 ?
K2A O5 K1 116.4(2) 22_565 18_655 ?
Nb1 O4 Nb2 114.5(3) . 6 ?
Nb1 O4 K2B 107.3(3) . 22_565 ?
Nb2 O4 K2B 93.5(3) 6 22_565 ?
Nb1 O4 K2A 97.6(2) . 22_565 ?
Nb2 O4 K2A 100.7(2) 6 22_565 ?
Nb1 O3 Nb1 94.1(2) 12_554 6 ?
Nb1 O3 Nb1 94.1(2) 12_554 . ?
Nb1 O3 Nb1 94.1(2) 6 . ?
Nb1 O3 Nb2 88.59(2) 12_554 12_554 ?
Nb1 O3 Nb2 88.21(2) 6 12_554 ?
Nb1 O3 Nb2 176.4(3) . 12_554 ?
Nb1 O3 Nb2 176.4(3) 12_554 6 ?
Nb1 O3 Nb2 88.59(3) 6 6 ?
Nb1 O3 Nb2 88.21(2) . 6 ?
Nb2 O3 Nb2 89.0(2) 12_554 6 ?
Nb1 O3 Nb2 88.21(2) 12_554 . ?
Nb1 O3 Nb2 176.4(3) 6 . ?
Nb1 O3 Nb2 88.59(3) . . ?
Nb2 O3 Nb2 89.0(2) 12_554 . ?
Nb2 O3 Nb2 89.0(2) 6 . ?
Nb1 O2 K1 129.3(3) . . ?
Nb1 O2 K1 96.7(2) . 18_655 ?
K1 O2 K1 109.7(2) . 18_655 ?
Nb1 O2 K2A 126.3(3) . . ?
K1 O2 K2A 82.8(2) . . ?
K1 O2 K2A 112.1(2) 18_655 . ?
Nb1 O2 K2B 117.9(3) . . ?
K1 O2 K2B 94.0(3) . . ?
K1 O2 K2B 108.5(3) 18_655 . ?
Nb2 O1 Nb2 116.1(3) 12_554 . ?
Nb2 O1 K2B 113.2(3) 12_554 20_565 ?
Nb2 O1 K2B 103.9(3) . 20_565 ?
Nb2 O1 K2A 102.8(2) 12_554 20_565 ?
Nb2 O1 K2A 108.8(3) . 20_565 ?
O2 K1 O6 101.3(2) . 4 ?
O2 K1 O2W 94.2(2) . 8_645 ?
O6 K1 O2W 147.1(2) 4 8_645 ?
O2 K1 O2 108.7(2) . 24_656 ?
O6 K1 O2 84.6(2) 4 24_656 ?
O2W K1 O2 117.7(2) 8_645 24_656 ?
O2 K1 O1W 104.1(2) . . ?
O6 K1 O1W 74.7(2) 4 . ?
O2W K1 O1W 73.4(2) 8_645 . ?
O2 K1 O1W 144.0(2) 24_656 . ?
O2 K1 O7 74.23(16) . 18_655 ?
O6 K1 O7 140.3(2) 4 18_655 ?
O2W K1 O7 71.9(2) 8_645 18_655 ?
O2 K1 O7 61.09(15) 24_656 18_655 ?
O1W K1 O7 145.06(19) . 18_655 ?
O2 K1 O1W 167.9(2) . 8_645 ?
O6 K1 O1W 90.00(19) 4 8_645 ?
O2W K1 O1W 73.8(2) 8_645 8_645 ?
O2 K1 O1W 76.54(19) 24_656 8_645 ?
O1W K1 O1W 74.4(3) . 8_645 ?
O7 K1 O1W 99.94(16) 18_655 8_645 ?
O2 K1 O5 125.60(17) . 24_656 ?
O6 K1 O5 122.95(19) 4 24_656 ?
O2W K1 O5 66.3(2) 8_645 24_656 ?
O2 K1 O5 53.09(15) 24_656 24_656 ?
O1W K1 O5 116.1(2) . 24_656 ?
O7 K1 O5 51.70(13) 18_655 24_656 ?
O1W K1 O5 48.42(16) 8_645 24_656 ?
O2 K1 Nb1 104.74(14) . 24_656 ?
O6 K1 Nb1 114.11(17) 4 24_656 ?
O2W K1 Nb1 89.26(19) 8_645 24_656 ?
O2 K1 Nb1 29.73(11) 24_656 24_656 ?
O1W K1 Nb1 147.23(19) . 24_656 ?
O7 K1 Nb1 36.60(10) 18_655 24_656 ?
O1W K1 Nb1 74.13(14) 8_645 24_656 ?
O5 K1 Nb1 31.69(9) 24_656 24_656 ?
O2 K1 K2A 52.77(16) . . ?
O6 K1 K2A 68.5(2) 4 . ?
O2W K1 K2A 99.9(2) 8_645 . ?
O2 K1 K2A 140.21(18) 24_656 . ?
O1W K1 K2A 56.6(2) . . ?
O7 K1 K2A 126.01(16) 18_655 . ?
O1W K1 K2A 129.73(17) 8_645 . ?
O5 K1 K2A 166.15(17) 24_656 . ?
Nb1 K1 K2A 155.96(12) 24_656 . ?
O2 K1 Na1 126.86(16) . . ?
O6 K1 Na1 106.41(17) 4 . ?
O2W K1 Na1 42.8(2) 8_645 . ?
O2 K1 Na1 118.23(14) 24_656 . ?
O1W K1 Na1 45.06(17) . . ?
O7 K1 Na1 107.28(13) 18_655 . ?
O1W K1 Na1 43.98(15) 8_645 . ?
O5 K1 Na1 72.21(10) 24_656 . ?
Nb1 K1 Na1 103.90(6) 24_656 . ?
K2A K1 Na1 97.76(12) . . ?
O2 K1 Nb1 19.89(13) . . ?
O6 K1 Nb1 97.33(15) 4 . ?
O2W K1 Nb1 106.4(2) 8_645 . ?
O2 K1 Nb1 88.94(13) 24_656 . ?
O1W K1 Nb1 122.25(18) . . ?
O7 K1 Nb1 64.90(10) 18_655 . ?
O1W K1 Nb1 163.08(14) 8_645 . ?
O5 K1 Nb1 115.55(11) 24_656 . ?
Nb1 K1 Nb1 88.96(5) 24_656 . ?
K2A K1 Nb1 67.17(11) . . ?
Na1 K1 Nb1 144.91(9) . . ?
O2W Na1 O2W 102.5(4) 8_645 11_556 ?
O2W Na1 O2W 102.5(4) 8_645 . ?
O2W Na1 O2W 102.5(4) 11_556 . ?
O2W Na1 O1W 167.9(4) 8_645 11_556 ?
O2W Na1 O1W 88.3(3) 11_556 11_556 ?
O2W Na1 O1W 80.2(3) . 11_556 ?
O2W Na1 O1W 88.3(3) 8_645 8_645 ?
O2W Na1 O1W 80.2(3) 11_556 8_645 ?
O2W Na1 O1W 167.9(4) . 8_645 ?
O1W Na1 O1W 88.2(3) 11_556 8_645 ?
O2W Na1 O1W 80.2(3) 8_645 . ?
O2W Na1 O1W 167.9(4) 11_556 . ?
O2W Na1 O1W 88.3(3) . . ?
O1W Na1 O1W 88.2(3) 11_556 . ?
O1W Na1 O1W 88.2(3) 8_645 . ?
O2W Na1 O4W 30.9(15) 8_645 18_655 ?
O2W Na1 O4W 83.9(16) 11_556 18_655 ?
O2W Na1 O4W 82.6(16) . 18_655 ?
O1W Na1 O4W 159.2(15) 11_556 18_655 ?
O1W Na1 O4W 109.4(15) 8_645 18_655 ?
O1W Na1 O4W 103.1(15) . 18_655 ?
O2W Na1 O4W 82.6(16) 8_645 21_656 ?
O2W Na1 O4W 30.9(15) 11_556 21_656 ?
O2W Na1 O4W 83.9(16) . 21_656 ?
O1W Na1 O4W 109.4(15) 11_556 21_656 ?
O1W Na1 O4W 103.1(15) 8_645 21_656 ?
O1W Na1 O4W 159.2(15) . 21_656 ?
O4W Na1 O4W 57(3) 18_655 21_656 ?
O2W Na1 O4W 83.9(16) 8_645 15_566 ?
O2W Na1 O4W 82.6(16) 11_556 15_566 ?
O2W Na1 O4W 30.9(15) . 15_566 ?
O1W Na1 O4W 103.1(15) 11_556 15_566 ?
O1W Na1 O4W 159.2(15) 8_645 15_566 ?
O1W Na1 O4W 109.4(15) . 15_566 ?
O4W Na1 O4W 57(3) 18_655 15_566 ?
O4W Na1 O4W 57(3) 21_656 15_566 ?
O2W Na1 K1 124.4(2) 8_645 11_556 ?
O2W Na1 K1 126.3(2) 11_556 11_556 ?
O2W Na1 K1 47.3(3) . 11_556 ?
O1W Na1 K1 49.35(18) 11_556 11_556 ?
O1W Na1 K1 121.7(2) 8_645 11_556 ?
O1W Na1 K1 58.02(19) . 11_556 ?
O4W Na1 K1 122.8(15) 18_655 11_556 ?
O4W Na1 K1 125.6(15) 21_656 11_556 ?
O4W Na1 K1 78.3(15) 15_566 11_556 ?
O2W Na1 K1 126.3(2) 8_645 8_645 ?
O2W Na1 K1 47.3(3) 11_556 8_645 ?
O2W Na1 K1 124.4(2) . 8_645 ?
O1W Na1 K1 58.02(19) 11_556 8_645 ?
O1W Na1 K1 49.35(18) 8_645 8_645 ?
O1W Na1 K1 121.7(2) . 8_645 ?
O4W Na1 K1 125.6(15) 18_655 8_645 ?
O4W Na1 K1 78.3(15) 21_656 8_645 ?
O4W Na1 K1 122.8(15) 15_566 8_645 ?
K1 Na1 K1 107.34(9) 11_556 8_645 ?
O2W Na1 K1 47.3(3) 8_645 . ?
O2W Na1 K1 124.4(2) 11_556 . ?
O2W Na1 K1 126.3(2) . . ?
O1W Na1 K1 121.7(2) 11_556 . ?
O1W Na1 K1 58.02(19) 8_645 . ?
O1W Na1 K1 49.35(18) . . ?
O4W Na1 K1 78.3(15) 18_655 . ?
O4W Na1 K1 122.8(15) 21_656 . ?
O4W Na1 K1 125.6(15) 15_566 . ?
K1 Na1 K1 107.34(9) 11_556 . ?
K1 Na1 K1 107.34(9) 8_645 . ?
Na1 O1W K1 85.6(2) . . ?
Na1 O1W K2A 147.0(3) . . ?
K1 O1W K2A 75.7(2) . . ?
Na1 O1W K1 78.0(2) . 11_556 ?
K1 O1W K1 163.4(3) . 11_556 ?
K2A O1W K1 119.8(2) . 11_556 ?
O4W O2W Na1 89(3) 15_566 . ?
O4W O2W K1 179(3) 15_566 11_556 ?
Na1 O2W K1 89.9(4) . 11_556 ?
O5W K2A O5W 92(3) . 22_565 ?
O5W K2A O3W 10(2) . . ?
O5W K2A O3W 86.0(11) 22_565 . ?
O5W K2A O3W 84.7(14) . 22_565 ?
O5W K2A O3W 10.8(17) 22_565 22_565 ?
O3W K2A O3W 79.3(11) . 22_565 ?
O5W K2A O2 112.3(17) . . ?
O5W K2A O2 112.2(13) 22_565 . ?
O3W K2A O2 108.5(7) . . ?
O3W K2A O2 122.3(9) 22_565 . ?
O5W K2A O1 160.1(17) . 23_665 ?
O5W K2A O1 77.0(14) 22_565 23_665 ?
O3W K2A O1 160.3(6) . 23_665 ?
O3W K2A O1 82.3(6) 22_565 23_665 ?
O2 K2A O1 87.4(2) . 23_665 ?
O5W K2A O5 122.0(16) . 19_656 ?
O5W K2A O5 112.7(14) 22_565 19_656 ?
O3W K2A O5 131.2(9) . 19_656 ?
O3W K2A O5 110.7(7) 22_565 19_656 ?
O2 K2A O5 105.1(3) . 19_656 ?
O1 K2A O5 50.69(18) 23_665 19_656 ?
O5W K2A O1W 87.9(16) . . ?
O5W K2A O1W 157.6(14) 22_565 . ?
O3W K2A O1W 96.5(8) . . ?
O3W K2A O1W 149.1(9) 22_565 . ?
O2 K2A O1W 88.2(2) . . ?
O1 K2A O1W 95.6(3) 23_665 . ?
O5 K2A O1W 50.13(19) 19_656 . ?
O5W K2A O4 110.7(17) . 19_656 ?
O5W K2A O4 64.5(14) 22_565 19_656 ?
O3W K2A O4 113.9(7) . 19_656 ?
O3W K2A O4 60.8(7) 22_565 19_656 ?
O2 K2A O4 136.9(3) . 19_656 ?
O1 K2A O4 49.54(17) 23_665 19_656 ?
O5 K2A O4 50.22(17) 19_656 19_656 ?
O1W K2A O4 94.5(2) . 19_656 ?
O5W K2A K2A 41.6(17) . 19_656 ?
O5W K2A K2A 91.2(12) 22_565 19_656 ?
O3W K2A K2A 48.9(8) . 19_656 ?
O3W K2A K2A 80.4(8) 22_565 19_656 ?
O2 K2A K2A 147.6(4) . 19_656 ?
O1 K2A K2A 120.8(3) 23_665 19_656 ?
O5 K2A K2A 84.7(2) 19_656 19_656 ?
O1W K2A K2A 74.3(3) . 19_656 ?
O4 K2A K2A 72.8(2) 19_656 19_656 ?
O5W K2A K2A 98.5(16) . 22_565 ?
O5W K2A K2A 34.8(13) 22_565 22_565 ?
O3W K2A K2A 89.2(8) . 22_565 ?
O3W K2A K2A 44.2(8) 22_565 22_565 ?
O2 K2A K2A 78.3(2) . 22_565 ?
O1 K2A K2A 82.5(3) 23_665 22_565 ?
O5 K2A K2A 132.2(3) 19_656 22_565 ?
O1W K2A K2A 166.4(3) . 22_565 ?
O4 K2A K2A 94.4(3) 19_656 22_565 ?
K2A K2A K2A 118.21(10) 19_656 22_565 ?
O5W K2A K1 90.2(17) . . ?
O5W K2A K1 154.6(13) 22_565 . ?
O3W K2A K1 93.0(5) . . ?
O3W K2A K1 161.7(7) 22_565 . ?
O2 K2A K1 44.42(15) . . ?
O1 K2A K1 106.7(2) 23_665 . ?
O5 K2A K1 86.91(19) 19_656 . ?
O1W K2A K1 47.68(16) . . ?
O4 K2A K1 137.1(2) 19_656 . ?
K2A K2A K1 107.1(3) 19_656 . ?
K2A K2A K1 119.9(3) 22_565 . ?
O5W K2B O3W 12(2) 22_565 22_565 ?
O5W K2B O5W 99(3) 22_565 . ?
O3W K2B O5W 89.8(13) 22_565 . ?
O5W K2B O3W 92.3(15) 22_565 . ?
O3W K2B O3W 84.1(12) 22_565 . ?
O5W K2B O3W 10.2(18) . . ?
O5W K2B O1 90.4(18) 22_565 23_665 ?
O3W K2B O1 95.4(7) 22_565 23_665 ?
O5W K2B O1 152.9(15) . 23_665 ?
O3W K2B O1 161.9(9) . 23_665 ?
O5W K2B O2 129.5(17) 22_565 . ?
O3W K2B O2 140.4(11) 22_565 . ?
O5W K2B O2 102.7(15) . . ?
O3W K2B O2 101.9(6) . . ?
O1 K2B O2 90.1(3) 23_665 . ?
O5W K2B O4 71.3(18) 22_565 19_656 ?
O3W K2B O4 66.5(8) 22_565 19_656 ?
O5W K2B O4 107.1(15) . 19_656 ?
O3W K2B O4 112.1(8) . 19_656 ?
O1 K2B O4 52.2(2) 23_665 19_656 ?
O2 K2B O4 139.8(4) . 19_656 ?
O5W K2B K2B 43.6(17) 22_565 22_565 ?
O3W K2B K2B 52.8(10) 22_565 22_565 ?
O5W K2B K2B 99.5(13) . 22_565 ?
O3W K2B K2B 89.3(8) . 22_565 ?
O1 K2B K2B 104.8(5) 23_665 22_565 ?
O2 K2B K2B 87.8(4) . 22_565 ?
O4 K2B K2B 112.7(4) 19_656 22_565 ?
O5W K2B K2B 95.8(16) 22_565 19_656 ?
O3W K2B K2B 83.6(10) 22_565 19_656 ?
O5W K2B K2B 34.1(15) . 19_656 ?
O3W K2B K2B 41.8(8) . 19_656 ?
O1 K2B K2B 120.1(5) 23_665 19_656 ?
O2 K2B K2B 126.6(5) . 19_656 ?
O4 K2B K2B 73.9(4) 19_656 19_656 ?
K2B K2B K2B 119.94(3) 22_565 19_656 ?
O5W K2B Nb2 66.1(18) 22_565 23_665 ?
O3W K2B Nb2 68.3(6) 22_565 23_665 ?
O5W K2B Nb2 137.1(15) . 23_665 ?
O3W K2B Nb2 140.1(7) . 23_665 ?
O1 K2B Nb2 29.20(14) 23_665 23_665 ?
O2 K2B Nb2 117.8(3) . 23_665 ?
O4 K2B Nb2 30.83(13) 19_656 23_665 ?
K2B K2B Nb2 95.6(4) 22_565 23_665 ?
K2B K2B Nb2 104.7(4) 19_656 23_665 ?
O5W K2B Nb2 114.3(18) 22_565 19_656 ?
O3W K2B Nb2 116.8(7) 22_565 19_656 ?
O5W K2B Nb2 132.1(14) . 19_656 ?
O3W K2B Nb2 142.4(9) . 19_656 ?
O1 K2B Nb2 25.65(14) 23_665 19_656 ?
O2 K2B Nb2 82.0(3) . 19_656 ?
O4 K2B Nb2 58.01(17) 19_656 19_656 ?
K2B K2B Nb2 128.3(4) 22_565 19_656 ?
K2B K2B Nb2 106.3(4) 19_656 19_656 ?
Nb2 K2B Nb2 48.65(11) 23_665 19_656 ?
O5W K2B K1 163.2(18) 22_565 . ?
O3W K2B K1 163.9(7) 22_565 . ?
O5W K2B K1 76.6(15) . . ?
O3W K2B K1 81.2(6) . . ?
O1 K2B K1 100.7(3) 23_665 . ?
O2 K2B K1 39.05(17) . . ?
O4 K2B K1 125.5(3) 19_656 . ?
K2B K2B K1 120.4(4) 22_565 . ?
K2B K2B K1 89.6(4) 19_656 . ?
Nb2 K2B K1 127.7(2) 23_665 . ?
Nb2 K2B K1 79.08(18) 19_656 . ?
O5W O3W K2B 48(9) . 19_656 ?
O5W O3W K2A 39(9) . . ?
O5W O3W K2B 50(9) . . ?
K2B O3W K2B 85.4(12) 19_656 . ?
O5W O3W K2A 57(9) . 19_656 ?
K2A O3W K2A 87.0(11) . 19_656 ?
O3W O5W K2B 119(10) . 19_656 ?
O3W O5W K2A 131(10) . . ?
O3W O5W K2B 119(10) . . ?
K2B O5W K2B 102(2) 19_656 . ?
O3W O5W K2A 112(10) . 19_656 ?
K2A O5W K2A 104(2) . 19_656 ?
O2W O4W Na1 60(3) 15_565 15_565 ?

_refine_diff_density_max         3.168
_refine_diff_density_min         -0.965
_refine_diff_density_rms         0.259

_shelxl_version_number           2013-4


_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_standards_number         0
_diffrn_standards_decay_%        0

